- Email: [email protected]

Contents lists available at ScienceDirect

Journal of Computational Physics journal homepage: www.elsevier.com/locate/jcp

Damage and fracture evolution in brittle materials by shape optimization methods Grégoire Allaire a,⇑, François Jouve b, Nicolas Van Goethem a,c a

Centre de Mathématiques Appliquées, École Polytechnique, 91128 Palaiseau, France Laboratoire J.-L. Lions, Université Paris Diderot (Paris 7), 75205 Paris, France c Universidade de Lisboa, Faculdade de Ciências, Departamento de Matemática, CMAF, Av. Prof. Gama Pinto, 1649-003 Lisboa, Portugal b

a r t i c l e

i n f o

Article history: Received 19 February 2010 Received in revised form 10 November 2010 Accepted 10 March 2011 Available online 21 March 2011 Keywords: Level set Shape optimization Damage Fracture

a b s t r a c t This paper is devoted to a numerical implementation of the Francfort–Marigo model of damage evolution in brittle materials. This quasi-static model is based, at each time step, on the minimization of a total energy which is the sum of an elastic energy and a Grifﬁth-type dissipated energy. Such a minimization is carried over all geometric mixtures of the two, healthy and damaged, elastic phases, respecting an irreversibility constraint. Numerically, we consider a situation where two well-separated phases coexist, and model their interface by a level set function that is transported according to the shape derivative of the minimized total energy. In the context of interface variations (Hadamard method) and using a steepest descent algorithm, we compute local minimizers of this quasi-static damage model. Initially, the damaged zone is nucleated by using the so-called topological derivative. We show that, when the damaged phase is very weak, our numerical method is able to predict crack propagation, including kinking and branching. Several numerical examples in 2d and 3d are discussed. Ó 2011 Elsevier Inc. All rights reserved.

1. Introduction Fracture mechanics is a ﬁeld of paramount importance which is the subject of intense research efforts, see [21,24,43] and reference therein. While many works address the issue of microscopic modelling of fractures and the coupling of some defect atomistic models with macroscopic elasto-plastic models, we focus on purely macroscopic models in the framework of continuum mechanics. Roughly speaking such continuum models can be classiﬁed in two main categories. On the one hand, there are models of crack growth and propagation which assume that the crack is a (d 1)-dimensional hypersurface in dimension d (a curve in the plane, and a surface in the three-dimensional space). On the other hand, one can consider models of damage where there is a competition between the initial healthy elastic phase and another damaged elastic phase. The transition from healthy to damaged can be smooth (i.e., there is a continuous damage variable which measures to what extent, or local proportion, the material is damaged) or sharp (i.e., there is an interface between a fully healthy and fully damaged zones). The Francfort–Marigo model [32] of quasi-static damage evolution for brittle materials pertains to the latter category and it is the purpose of this work to propose a numerical implementation of such a model. One of our main conclusion is that, although the Francfort–Marigo model is a damage model, it is able to describe crack propagation, when the damaged phase is very weak, and it gives quite similar results to those obtained in [20,21]. This is

⇑ Corresponding author. E-mail addresses: [email protected] (G. Allaire), [email protected] (F. Jouve), [email protected] (N. Van Goethem). 0021-9991/$ - see front matter Ó 2011 Elsevier Inc. All rights reserved. doi:10.1016/j.jcp.2011.03.024

G. Allaire et al. / Journal of Computational Physics 230 (2011) 5010–5044

5011

not so much a surprise (although not a proof, of course) since the numerical approach in these papers is based on a Cconvergence approximation (à la Ambrosio-Tortorelli) which amounts to replace the original fracture model by a damage model. Section 2 gives a complete description of the Francfort–Marigo damage model that we brieﬂy summarize now. A smooth body X Rd (d = 2, 3) is ﬁlled with two elastic phases: the undamaged or ‘‘healthy’’ phase, and the damaged one which is much weaker. The damaged zone is X0 X, with characteristic function v(x), and the healthy zone is the remaining region X1 = XnX0. The behavior of such a mixture is assumed to be linearly elastic with a perfect interface (i.e., natural transmission conditions take place at the interface). Starting from an initial conﬁguration of damaged and healthy phases mixture vinit(x) and for a given set of loads, the new damaged conﬁguration vopt(x) is obtained by minimizing a total energy

JðvÞ ¼ J elast ðvÞ þ j

Z

v dV;

ð1:1Þ

X

which is the sum of the elastic energy and a Grifﬁth-like bulk energy for the creation of the damaged region (where j > 0 is a material parameter representing the energy density released at the onset of damage), under an irreversibility constraint which forbids an initially damaged zone to become healthy anew, i.e.,

vðxÞ P vinit ðxÞ: A quasi-static damage evolution model is then obtained by a time discretization of the force loading and by applying the previous constrained minimization at each time step. For numerical purposes we represent the interface R between the damaged and healthy regions, X0 and X1, respectively, by a level set function. The level set method for front propagation, as introduced by Osher and Sethian [50], is well-known to be very convenient for this purpose, including the possibility of topology changes. Here, we take advantage of another feature of the level set method, namely the local character of front displacement. In other words, we do not seek global minimizers of (1.1) but rather local minimizers obtained from the initial conﬁguration vinit by transporting it using the level set method. Although global minimization is the ultimate goal in many optimization problems (like, for example, shape optimization [3,5]), it turns out to be an undesirable feature in the present problem of damage evolution. Indeed, as explained in [20], global minimization is mechanically not sound for a quasi-static evolution problem where meta-stable states should be preferred to globally stable states attained by crossing a high energy barrier. In the context of the level set method, at each time step, the new damage conﬁguration vopt is obtained from the initialization vinit by solving a transport Hamilton–Jacobi equation with a normal velocity which is minus the shape derivative of the total energy (1.1). Section 3 is devoted to the computation of such a shape derivative, following Hadamard method of geometric optimization (see e.g. [3,38,46,59]). Remark that this computation is not standard (and indeed new in the elasticity context, to the best of our knowledge) since it is an interface between two materials, rather than a boundary, which is moved and since the full strain and stress tensors are not continuous through the interface. Note however that, for continuous ﬁelds, the derivation with respect to the shape of an interface is already known, see e.g. [53,60]. The numerical algorithm for the level set method is by now standard and is brieﬂy recalled in Section 6. One of the inconveniences of the level set method, as well as of most numerical methods for crack propagation, is its inability to nucleate damage and start a front evolution if there is no initial interface. Therefore, we use another ingredient to initialize our computations when no initial damaged zone is prescribed. Namely, we use the notion of topological derivative as introduced in [30,34,58], and applied to the case of elastic inclusions in [8,9,17] for inverse problems, and to cracks in [61]. The topological derivative aims at determining whether it is worth or not nucleating an inﬁnitesimal damage inclusion in the healthy zone X1. This information is complementary to that obtained by shape variation since, on the one hand, the shape derivative cannot nucleate new inclusions and, on the other hand, once an inclusion is created, only the shape derivative can expand it further on. The notion of topological derivative will be detailed in Section 4. The resulting numerical algorithm is somehow similar to previous algorithms in structural optimization [5,62]. When the damaged phase is much weaker than the healthy phase (say, with a 103 ratio between the Young moduli) and for a suitably chosen Grifﬁth energy release parameter j (which scales like the inverse of the mesh size Dx), our numerical results are very similar to those of [20] which were obtained for a fracture model. Therefore we claim that our numerical implementation of the Francfort–Marigo damage model is able to simulate crack propagation. Numerical experiments, including a study of convergence under mesh reﬁnement, are performed in Section 6. We believe our approach is simpler and computationally less intensive than other classical methods for crack propagation [1,13,16,36,37,47,48]. Let us emphasize that level-set methods have already been used in fracture mechanics [18,36,37], usually in conjunction with the extended ﬁnite element method [44]. However, one novelty of our work is that we use a single level-set function instead of two for parametrizing the crack and that the weak damage phase avoids the use of discontinuous ﬁnite elements. After completion of this work we learned that similar ideas were independently introduced in [14,42]. A different approach, called eigen deformation, was recently proposed in [56]: it uses two ﬁelds, like in [20], and relies on a scaling resembling ours (see (2.11) below). Eventually Section 7 draw some conclusions on our numerical experiments which yield comparable but different results from those obtained by the back-tracking algorithm for global minimization proposed in [19,21]. Our results, including some computations in 2d, were announced in [6].

5012

G. Allaire et al. / Journal of Computational Physics 230 (2011) 5010–5044

2. The Francfort–Marigo model of damage 2.1. Description of the model This section gives a comprehensive description of the Francfort–Marigo model [32] of quasi-static damage evolution for brittle materials. In a smooth domain X Rd this damage model is stated as a macroscopic phase transition problem between a damaged phase occupying a subset X0 X and an healthy phase in the remaining region X1 = XnX0. To simplify the presentation, in a ﬁrst step we consider a static problem starting from a healthy conﬁguration (namely, without any irreversibility constraint). The characteristic function of X0 is denoted by v(x). The healthy and damaged phases are both assumed to be linear, isotropic and homogeneous, so we work in a linearized elasticity framework and the Lamé tensor of elasticity in X is

Av ¼ A1 ð1 vÞ þ A0 v; where 0 < A0 < A1 are the Lamé tensors of isotropic elasticity in the damaged and healthy regions, respectively, deﬁned by

A0;1 ¼ 2l0;1 I4 þ k0;1 I2 I2 ; where I2 and I4 denote the identity 2nd and 4th order tensors, respectively. The boundary of the body is made of two parts, @ X = CD [ CN, where a Dirichlet boundary condition uD is imposed on CD and a Neumann boundary condition g is imposed on CN. We assume that uD 2 H1 ðX; Rd Þ, g 2 L2 ð@ X; Rd Þ and we consider also a body force f 2 L2 ðX; Rd Þ. (Slightly stronger regularity assumptions on the data f, g, uD will be made in the sequel.) We denote by n the unit normal vector on @ X. We introduce the afﬁne space of kinematically admissible displacement ﬁelds

V ¼ fu 2 H1 ðX; Rd Þ such that u ¼ uD on CD g: As usual, the strain and stress tensors associated to a displacement u write as

eðuÞ ¼

1 ðru þ rT uÞ; 2

rðuÞ ¼ Av eðuÞ:

ð2:1Þ

The elasticity system reads as

8 > < divðAv eðuv ÞÞ ¼ f uv ¼ uD > : Av eðuv Þn ¼ g

in X; on CD ;

ð2:2Þ

on CN :

It is well-known that (2.2) can be restated as a minimum potential energy principle, that is, the displacement ﬁeld uv 2 V minimizes in V the energy functional

P v ðuÞ ¼

Z Z 1 Av eðuÞ eðuÞ f u dV g u dS; X 2 CN

i.e.,

P v ðuv Þ ¼ min P v ðuÞ: u2V

The Francfort–Marigo model amounts to minimize jointly over u and v a total energy which is the sum of the elastic potential energy and of a Grifﬁth-type energy (accounting for the creation of the damaged region), writing as

J ðu; vÞ ¼ P v ðuÞ þ j

Z

v dV;

ð2:3Þ

X

where j is a positive material parameter which represents the release of elastic energy due to the decrease of rigidity at the onset of damage and can be interpreted as a density of dissipated energy of the damaged region. We call j the Grifﬁth energy release parameter. In other words, the Francfort–Marigo model is based on the minimization over v 2 L1(X;{0, 1}) of

JðvÞ ¼ J ðuv ; vÞ ¼ min J ðu; vÞ: u2V

ð2:4Þ

Instead of writing (2.4), we can ﬁrst minimize in v and later in u (since (2.3) is doubly minimized, the order of minimization does not matter). Since v(x) takes only the values 0 and 1, the minimization is easy, provided that we know uv (which is of course never the case). Indeed, minimizing (2.4) is equivalent to the following local minimization at each point x 2 X

1 Av eðuv Þ eðuv Þ þ jv ðxÞ; v2f0;1g 2 min

providing a transition criterion from the healthy to the damaged phase as soon as the release of elastic energy is larger than the threshold j. More precisely, a point x is damaged if and only if

1 1 1 A eðuv Þ eðuv ÞðxÞ A0 eðuv Þ eðuv ÞðxÞ P j: 2 2

ð2:5Þ

G. Allaire et al. / Journal of Computational Physics 230 (2011) 5010–5044

5013

After minimization in v we obtain a non-linear non-convex functional to be minimized in V

EðuÞ ¼

1 2

Z

Z Z min A1 eðuÞ eðuÞ; A0 eðuÞ eðuÞ þ 2j dV f u dV

X

X

g u dS:

ð2:6Þ

CN

In truth the Francfort–Marigo model is quasi-static which means that we consider a sequence of minimization problems of the above type, with an additional thermodynamic irreversibility constraint. The time is discretized by an increasing sequence (ti)iP1, with t1 = 0 and ti < ti + 1. At each time ti the loads are denoted by fi and gi, the imposed boundary displacement is uD, i, the afﬁne space of kinematically admissible displacement ﬁelds is Vi, the characteristic function of the damaged phase is vi and the corresponding displacement is uvi , solution of (2.2) with loads fi and gi and Dirichlet boundary condition uD, i. The initial damaged zone is given and characterized by v0. The model is irreversible which means that a material point x 2 X which is damaged at a previous time must remain damaged at a later time ti, i.e.,

vi ðxÞ P vi1 ðxÞ:

ð2:7Þ

Therefore, introducing J i and Ji, which are deﬁned as (2.3) and (2.4) with the loads at time ti, the Francfort–Marigo model is a sequence, indexed by i P 1, of minimization problems

inf

v2L1 ðX;f0;1gÞ; vPvi1

J i ðvÞ ¼

inf

u2V i ;v2L1 ðX;f0;1gÞ; vPvi1

J i ðu; vÞ;

ð2:8Þ

with minimizers vi and uvi (if any). 2.2. Mathematical properties of the model The Francfort and Marigo model is ill-posed, namely, there does not exist any minimizer of (2.8) in most cases. This can easily be seen because (2.8) is equivalent to the minimization of the non-linear elastic energy (2.6) which is not convex, neither quasi-convex. Actually, one of the main purposes of the seminal paper [32] of Francfort and Marigo was to relax the minimization problem (2.8) and show the existence of suitably generalized solutions. The relaxation of (2.8) amounts to introduce composite materials, obtained by a ﬁne mixing of the two phases, as competitors in the minimization of the total energy. Such composite materials include the limits, in the sense of homogenization, of minimizing sequences of (2.8): they are characterized by a phase volume fraction in the range [0,1_] and a homogenized elasticity tensor which is the output of the microstructure at given volume fractions. It turns out that optimal microstructures are found in the class of sequential laminates. For further details we refer to [32] for the ﬁrst time step and to [31] for the following time steps (where the irreversibility constraint plays a crucial role). This relaxed approach has been used for numerical computations of damage evolution in [4]. One drawback of the Francfort–Marigo approach is that it relies on global minimization, i.e., at each time step ti the functional J i ðu; vÞ is globally minimized with respect to both variables u and v. There is no true mechanical motivation for insisting on global minimization with respect to v. Because of global minimization, damage might occur at time step ti in a region far away from the initially damaged zone at the previous time step ti1, whereas, in most circumstances, it seems more natural from a physical viewpoint to have expansion of the previously damaged area. Therefore, in a quasi-static regime which may favor metastability effects, it seems reasonable to prefer local minimization (with respect to v) instead of global minimization. In the context of fracture mechanics it was proved in [48] that criticality solutions of the Grifﬁth model are different from the energy globally minimizing solutions proposed by Francfort and Marigo. Unfortunately, for a scalar-valued version of our damage model (antiplane elasticity), it was recently proved in [35] that local minima are actually global ones (both in the original setting of characteristic functions or in the relaxed setting of composite materials, locality being evaluated in the L1(X)-norm). However this last result of [35] does not prevent the possibility of a different framework in which local minimizers would not be global ones (see, for example, the notion of e-stable minimizer in [41]). In the present paper we propose such a framework based on the notion of front propagation in the original case of a macroscopic distribution of healthy and damaged phases (i.e., not considering composite materials). Instead of representing a damaged zone by a characteristic function v 2 L1(X;{0, 1}) we rather introduce the interface R between the healthy and the damaged regions. Admissible variations of this interface are obtained in the framework of Hadamard method of shape variations [3,38,46,52,59] (see Section 3 below). More precisely, the minimization in (2.8) is restricted to conﬁgurations which are obtained by a Lipschitz diffeomorphism from a reference or an initial conﬁguration. This is a severe restriction of the space of admissible designs since, for example, all conﬁgurations share the same topology as the reference one. As a consequence there cannot be nucleation of new damaged zones away from the initial one. This leaves open the possibility of the existence of local, but not global, minimizers. We shall not prove anything rigorously on this issue but our numerical simulations indicate that they do indeed exist. Let us remark that the chosen numerical approach by level sets allows for topology changes by breaking a damage region in two parts, but never by creating a new damage region. On the other hand, working in the framework of Hadamard method of front representation does not help at all concerning the existence of (local or global) minimizers. Once again we are speechless on this issue. Of course, one simple remedy is to add a surface energy in the minimized total energy

J reg ðu; vÞ ¼ P v ðuÞ þ j

Z X

v dV þ j0 TVðvÞ;

ð2:9Þ

5014

G. Allaire et al. / Journal of Computational Physics 230 (2011) 5010–5044

with the total variation norm deﬁned by

TVðvÞ ¼

Z

sup /2C 1 ðX;Rd Þ j/j61 in X

vdiv/ dV:

X

When v is the characteristic function of a smooth subset X0, the number TV(v) is also the perimeter of X0. A possible justiﬁcation of this new term in (2.9) is to consider a Grifﬁth surface energy on top of the previous Grifﬁth bulk energy. We call ‘‘regularized’’ the energy in (2.9) since it is well-known to admit minimizers v in the class L1(X;{0, 1}) [12]. In truth, if we mention this additive surface energy, this is because the unavoidable numerical diffusion of our computational algorithm has precisely the effect of adding such a surface energy. For our numerical tests, we shall not rely on (2.9) and rather we use the standard energy (2.3). 2.3. Goal of the present study The goal of this paper is to propose and test the following numerical method for the damage model of Francfort and Marigo. At each time step ti the minimization (2.8) is performed by Hadamard method of shape sensitivity. In other words, we compute the shape derivative of the objective function Ji with respect to the interface between the healthy and damaged phases and, applying a steepest descent algorithm, we move this interface in (minus) the direction of the shape gradient. The minimization of Ji is stopped when the shape gradient is (approximately) zero, i.e., at a stationary point (a local minimizer in numerical practice) of the objective function. We use a level set approach to characterize the interface between the healthy and damaged phases. As is well known, it allows for large deformations of the interface with possibly topology changes. After convergence at time ti, we pass to the next discrete time ti+1 by changing the loads and we start a new minimization of Ji+1, taking into account the irreversibility constraint (2.7). We iterate until a ﬁnal time t ifinal which we choose when the structure is almost entirely damaged. We propose two possible ways of initializing our computations. Either we start from an initial damaged zone v0 at time t1 = 0, or, in case the initial structure is not damaged at all, we nucleate a small damaged zone by using the notion of topological derivative. This nucleation step takes place before we start the ﬁrst minimization of J1. In particular, the resulting initial damaged zone is usually not a local minimizer of the total energy (2.3). We are thus able to predict damage propagation without prescribing any initial crack as is commonly done in engineering practice. Although the considered model has been designed in the framework of damage mechanics, it turns out to be able to accurately describe crack propagation in some speciﬁc regimes. More precisely, when the damaged phase is very weak (its rigidity A0 is negligible) and the energy release rate is large enough, the results of our numerical computations are cracks rather than damaged sub-domains. In other words, the damaged zone is a thin hypersurface with a thickness of a few mesh cells concentrating along a curve in 2d or a surface in 3d. However, our model, based on the minimization of (2.3), has no intrinsic lengthscale as opposed to other fracture models where there is a competition between bulk (elastic) energy and surface (crack extension) energy [21]. Therefore we must introduce some characteristic lengthscale in our model if we want to support our claim that it is able to predict crack propagation. We do this at a numerical level by requiring that our fracture results are convergent under mesh reﬁnement, a necessary condition for any reasonable numerical algorithm. To obtain such a convergence we scale the Grifﬁth bulk energy release parameter j like 1/Dx, where Dx is the mesh size which is reﬁned. More precisely, we introduce a characteristic lengthscale ‘ and we deﬁne a new material parameter c which can be thought of as a Grifﬁth surface energy release parameter (or fracture toughness in the language of fracture mechanics)

c ¼ j‘:

ð2:10Þ

Then, instead of minimizing (2.3), we minimize (assuming, for simplicity, that there are only bulk forces)

J Dx ðu; vÞ ¼

Z X

Z 1 c v dV; Av eðuÞ eðuÞ f u dV þ 2 Dx X

ð2:11Þ

where c/Dx has the same physical units than j. Although (2.11) has been written in a continuous framework, we are actually interested in its discretized version for a mesh of size Dx obtained, for example, with piecewise afﬁne continuous Lagrange ﬁnite elements for u and piecewise constant ﬁnite elements for v. In other words, rather than (2.11) we consider

J Dx ðuDx ; vDx Þ ¼

Z Z 1 c Av eðuDx Þ eðuDx Þ f uDx dV þ v dV; Dx X Dx X 2

ð2:12Þ

where the minimization carries over the ﬁelds uDx and vDx belonging to the above ﬁnite element spaces (of ﬁnite dimension, linked to the mesh size Dx). When Dx goes to zero, we expect that, for a minimizing sequence vDx, the last term of (2.11) converges to a surface energy

lim

Dx!0

c Dx

Z X

vDx dV ¼ c

Z C

dS;

G. Allaire et al. / Journal of Computational Physics 230 (2011) 5010–5044

5015

where C is the crack curve in 2d or surface in 3d. The numerical examples of Section 6 show that it is indeed the case: the damage zone concentrates around a surface C with a thickness of a few cells Dx. We believe that the discrete scaled energies (2.12) converges, in some sense to be made precise, as Dx and A0 go to zero, to the fracture model

min

Z 1 dS; A1 eðuÞ eðuÞ f u dV þ c XnC 2 C

Z

u;C

ð2:13Þ

where the displacement ﬁeld u may be discontinuous through the crack C. We are not able to prove such a result which would ﬁrst require to order the speed of convergence of Dx and A0 to zero. Remark however that similar results of convergence of a sequence of discrete energies to a continuous limit energy have already been obtained, e.g. in the context of image segmentation for discrete Mumford–Shah energies [27] or for spin systems [23]. A natural candidate for the type of convergence of (2.12) to (2.13) would be of course C-convergence. However, since our numerical approach relies on some type of local minimizers, whereas C-convergence only deals with global minimizers, one should pertain to a variant of C-convergence for ‘‘local minimizers’’ (a notion to be made precise) as in the recent works [22,40,55]. Although a convergence of (2.12) to (2.13) would probably be difﬁcult and quite technical to prove, our numerical results are a clear indication that it may hold true. This conjectured link between the damage model (2.11) and the fracture model (2.13) is, of course, reminiscent (but not equivalent) of the numerical approach in [20,21] where a fracture model is numerically approximated by a damage model (based on the C-convergence result of [7]). 3. Shape derivative 3.1. On the notion of shape gradient Shape differentiation is a classical topic [3,38,46,52,59]. We brieﬂy recall its deﬁnition and main results in the present context. Here, the overall domain X is ﬁxed and we consider a smooth open subset x X which may vary. Denoting by v the characteristic function of x, we consider variations of the type

vh ¼ v ðId þ hÞ; i:e:; vh ðxÞ ¼ vðx þ hðxÞÞ; with h 2 W 1;1 ðX; Rd Þ such that h is tangential on @ X (this last condition ensures that X = (Id + h)X). It is well known that, for sufﬁciently small h, (Id + h) is a diffeomorphism in X. Deﬁnition 3.1. The shape derivative of a function J(v) is deﬁned as the Fréchet derivative in W 1;1 ðX; Rd Þ at 0 of the application h ? J(v(Id + h)), i.e.

Jðv ðId þ hÞÞ ¼ JðvÞ þ J 0 ðvÞðhÞ þ oðhÞ with

lim h!0

joðhÞj ¼ 0; khkW 1;1

where J0 (v) is a continuous linear form on W 1;1 ðX; Rd Þ. Lemma 3.1 ([38,59]). Let x be a smooth bounded open subset of X and h 2 W 1;1 ðX; Rd Þ. Let f 2 H1(X) and g 2 H2(X) be two given functions. Assume that R is a smooth subset of @ x with boundary @ R. The shape derivatives of

J 1 ð xÞ ¼ are J 01 ðxÞ ¼

R

Z x

@x

J 02 ðRÞ ¼

f dV

and J 2 ðRÞ ¼

Z

g dS

R

f h n dS and

Z R

Z @g þ gH h n dS þ g h s dL; @n @R

ð3:1Þ

respectively, where n is the exterior unit vector normal to @ x, H is the mean curvature and s is the unit vector tangent to @ x such that s is normal to both @ R and n, and dL is the (d 2)-dimensional measure along @ R. 3.2. Main result To simplify the notations we forget the time index ti in this section. Although the state equation and the cost function of the Francfort–Marigo model are (2.2) and (2.4), respectively, we consider a slightly more general setting in this section (to pave the way to more general models in the future). More precisely, we consider a state equation

8 > < divðAv eðuv ÞÞ ¼ fv uv ¼ uD > : Av eðuv Þn ¼ g v

in X; on CD ; on CN ;

ð3:2Þ

5016

G. Allaire et al. / Journal of Computational Physics 230 (2011) 5010–5044

where

fv :¼ ð1 vÞf 1 þ vf 0

and g v :¼ ð1 vÞg 1 þ vg 0

with f k 2 H1 ðX; Rd Þ \ C 0;a ðX; Rd Þ and g k 2 H2 ðX; Rd Þ \ C 1;a ðX; Rd Þ, k = 0 or 1 (0 < a < 1). We also assume that uD belongs to H2 ðX; Rd Þ and that the subset X0 (with characteristic function v) is smooth. Under these assumptions the solution uv of (3.2) belongs to H2 ðX0 ; Rd Þ and H2 ðX1 ; Rd Þ and is of class C 2;a away from the boundary and from the interface. The cost function is taken as

JðvÞ ¼

Z

1 2

Av eðuv Þ eðuv ÞdV þ

Z

X

X

jv ðx; uv ÞdV þ

Z

hv ðx; uv ÞdS; ;

ð3:3Þ

@X

where 1

jv :¼ ð1 vÞj þ vj

1

0

and hv :¼ ð1 vÞh þ vh

0

with jk(x, u) and hk(x, u), k = 0, 1, twice differentiable functions with respect to u, satisfying the following growth conditions k

k

jj ðx; uÞj 6 Cðjuj2 þ 1Þ;

k

jðj Þ0 ðx; uÞj 6 Cðjuj þ 1Þ;

k

jðj Þ00 ðx; uÞj 6 C;

k

jh ðx; uÞj 6 Cðjuj2 þ 1Þ;

jðh Þ0 ðx; uÞj 6 Cðjuj þ 1Þ;

k

jðh Þ00 ðx; uÞj 6 C:

ð3:4Þ

where 0 denotes the partial derivative with respect to u 2 Rd . To avoid some unnecessary technicalities we also assume that h1(x, uD (x)) = h0(x, uD(x)) on CD so that the objective function is equal to

JðvÞ ¼

Z

1 2

Av eðuv Þ eðuv ÞdV þ

X

Z X

jv ðx; uv ÞdV þ

Z

hv ðx; uv ÞdS þ C;

CN

where C is a constant which does not depend on v. Remark 3.1. When the imposed displacement on CD vanishes, uD = 0, the cost function of the Francfort–Marigo model simpliﬁes and reduces to a multiple of the compliance. Indeed, the energy equality for the state Eq. (2.2) (which is valid only if uD = 0), namely

Z

Av eðuv Þ eðuv Þ dV ¼

Z

X

f uv dV þ

Z

g uv dS; CN

X

implies that the cost function (2.4) (with jv = jv fuv and gv = guv) reduces to

JðvÞ ¼ j

Z

v dV

X

1 2

Z

X

f uv dV þ

Z

g uv dS :

ð3:5Þ

CN

Of course, the study of (3.5) is much simpler than that of the general objective function (3.3). However, since many numerical tests involve non-homogeneous boundary displacements, uD – 0, we must study (3.3) and not merely (3.5). We need to introduce the so-called adjoint problem

8 0 > < divðAv eðpv ÞÞ ¼ fv þ jv ðx; uv Þ in X; pv ¼ 0 on CD ; > : 0 on CN : Av eðpv Þn ¼ g v þ hv ðx; uv Þ

ð3:6Þ

We denote by R the interface between the damaged and healthy regions X0 and X1. We deﬁne n = n0 = n1 the outward unit normal vector to R. We use the jump notation

½a ¼ a1 a0

ð3:7Þ

for a quantity a that has a jump across the interface R. The shape derivative of (3.3) will be an integral on the interface R as is clear from Lemma 3.1. The state uv and adjoint pv are continuous on R but not all their derivatives. Actually the tangential components of their deformation tensors are continuous as well as the normal vector of their stress tensors. To make this result precise, at each point of the interface R we introduce a local basis made of the normal vector n and a collection of unit tangential vectors, collectively denoted by t, such that (t, n) is an orthonormal basis. For a symmetric d d matrix M, written in this basis, we introduce the following notations

M¼

Mtt

Mtn

Mnt

Mnn

;

where Mtt stands for the (d 1) (d 1) minor of M, Mtn is the vector of the (d 1) ﬁrst components of the d-th column of M, Mnt is the row vector of the (d 1) ﬁrst components of the d-th row of M, and Mnn the (d, d) entry of M. Let us recall

5017

G. Allaire et al. / Journal of Computational Physics 230 (2011) 5010–5044

that dV, dS and dL indicate volume integration in Rd , and surface (or line, according to the value of d) integration in Rd1 and Rd2 , respectively. Lemma 3.2. Let e and r denote the strain and stress tensors of the solution to the state Eq. (3.2) or adjoint state Eq. (3.6). All components of rnt, rnn, and ett are continuous across the interface R (assumed to be smooth) while all other entries have jumps through R, rewritten in terms of these continuous quantities as

8 1 1 > < ½enn ¼ ½ð2l þ kÞ rnn ½kð2l þ kÞ trett ; 1 ½etn ¼ ½ð2lÞ rtn ; > : ½rtt ¼ ½2lett þ ð½2lkð2l þ kÞ1 trett þ ½kð2l þ kÞ1 rnn ÞId1 2 ;

ð3:8Þ

where Id1 is the identity matrix of order d 1. 2 Proof. By standard regularity theory, on both sides of the smooth interface R the solution, as well as its deformation and stress tensors e and r, are smooth. This implies that the continuity of the displacement through the interface yields the continuity of ett. The transmission condition implies that rtn and rnn are also continuous on the interface. The other quantities have jumps (3.8) which are computed through the strain–stress relation (2.1). h Theorem 3.1. Let X be a smooth bounded open set, R be a smooth hypersurface in X, c = R \ CN and h 2 W 1;1 ðX; Rd Þ. The shape derivative in the direction h of the objective function J(v), as given by (3.3), is

J 0 ðvÞðhÞ ¼

Z

DðxÞ h n dS þ

R

Z Z 0 1 0 1 ðf 0 f 1 Þ pv þ ðj j Þðx; uv Þ h n dS þ ðg 0 g 1 Þ pv þ ðh h Þðx; uv Þ h s dL R

c

ð3:9Þ with

1 1 2kl rnn ðuv Þrnn ðpv Þ rtn ðuv Þ rtn ðpv Þ þ ½2lett ðuv Þ ett ðpv Þ þ trett ðuv Þtrett ðpv Þ ðk þ 2lÞ l ðk þ 2lÞ k 1 1 þ jrtn ðuv Þj2 ðrnn ðuv Þtrett ðpv Þ þ rnn ðpv Þtrett ðuv ÞÞ þ ðrnn ðuv ÞÞ2 þ ðk þ 2lÞ 2ðk þ 2lÞ 2l 2 kl

k trett ðuv Þ ½ljett ðuv Þj2 rnn ðuv Þtrett ðuv Þ; k þ 2l k þ 2l

DðxÞ ¼

ð3:10Þ

where uv and pv are the solutions of the state Eq. (3.2) and adjoint Eq. (3.6), respectively, and where the brackets denotes the jump as deﬁned by (3.7). Equivalently, DðxÞ can be rewritten as

DðxÞ ¼ rnn ðuv Þ½enn ðpv Þ þ ett ðuv Þ ½rtt ðpv Þ 2½etn ðuv Þ rtn ðpv Þ þ

1

rnn ðuv Þ½enn ðuv Þ ett ðuv Þ ½rtt ðuv Þ þ 2rtn ðuv Þ ½etn ðuv Þ : 2

ð3:11Þ

Remark 3.2. A formula, partially symmetric to (3.11), holds true

DðxÞ ¼ rnn ðpv Þ½enn ðuv Þ þ ett ðpv Þ ½rtt ðuv Þ 2½etn ðpv Þ rtn ðuv Þ þ

1

rnn ðuv Þ½enn ðuv Þ ett ðuv Þ ½rtt ðuv Þ þ 2rtn ðuv Þ ½etn ðuv Þ : 2

ð3:12Þ

The main interest of (3.11), or (3.12), compared to (3.10), is that it does not involve jumps of the Lamé coefﬁcients which blow up when the damaged phase degenerate to zero. Indeed, it is interesting to investigate the limit of the shape derivative in Theorem 3.1 when A0 converges to zero. In such a case, we recover previously known formulas, used in shape optimization [3,38,59]. As A0 tends to zero, it is well known that, on the interface R, the normal stress rn = (rtn, rnn) converges also to zero, while the deformation tensor e remains bounded. Therefore, the limit formula of (3.11), or (3.12), is

1 DðxÞ ¼ ett ðuv Þ rtt ðpv Þ ett ðuv Þ rtt ðuv Þ: 2

ð3:13Þ

The proof of Theorem 3.1 is given in the next subsection (except some technical computations which are postponed to Appendix A). Similar results in the conductivity setting (scalar equations) appeared in [15,39,51]. Let us now restate Theorem 3.1 for the Francfort–Marigo cost function, in which case we have k

j ðx; uÞ ¼ f k uk þ jdk0

and hk ðx; uÞ ¼ g k uk ;

where dk0 is the Kronecker symbol, equal to 0 if k = 1 and to 1 if k = 0. It turns out that the problem is self-adjoint, i.e., there is no need of an adjoint state. More precisely, in this context we ﬁnd that pv = 0. We further simplify the previous Theorem 3.1 by taking forces which are the same in the damaged and healthy regions, i.e., f0 = f1 and g0 = g1. Then, we obtain

5018

G. Allaire et al. / Journal of Computational Physics 230 (2011) 5010–5044

Corollary 3.1. Let f0 = f1 and g0 = g1. The shape derivative of (2.4) in the direction h is

J 0 ðvÞðhÞ ¼

Z

DðxÞh n dS

R

with

1

rnn ðuv Þ½enn ðuv Þ ett ðuv Þ ½rtt ðuv Þ þ 2rtn ðuv Þ ½etn ðuv Þ : 2 Furthermore, if A0 6 A1, then ðDðxÞ jÞ 6 0 on R. DðxÞ ¼ j þ

ð3:14Þ

The last result of Corollary 3.1 implies that, upon neglecting the Grifﬁth energy release rate, i.e. taking j = 0, one should take h n P 0 to get a negative shape derivative. In other words, the damaged phase should ﬁll the entire domain in order to minimize the energy functional (2.4) (which is clear from the minimization (2.5)). 3.3. The Lagrangian approach to shape differentiation This section is devoted to the proof of Theorem 3.1 by means of a Lagrangian method which, in the context of shape optimization, is described in e.g. [3,5,26]. It amounts to introduce a Lagrangian which, as usual, is the sum of the objective function and of the constraints multiplied by suitable Lagrange multipliers. In shape optimization the state equation is seen as a constraint and the corresponding Lagrange multiplier is precisely the adjoint state at optimality. The shape derivative J0 (v)(h) is then obtained as a simple partial derivative of the Lagrangian L. This approach is also very convenient to guess the exact form of the adjoint problem. In the present setting it is the shape of the subdomains X0 and X1 which is varying, or equivalently the interface R. Differentiating with respect to the position of this interface is more complicated than differentiating with respect to the outer boundary as in usual shape optimization problems. The additional difﬁculty, which was recognized in [51] (see also [15,39]) is that the solution uv of the state Eq. (3.2) is not shape differentiable in the sense of Deﬁnition 3.1. The reason is that some spatial derivatives of uv are discontinuous at the interface (because of the jump in the material properties): thus, when we additionally differentiate with respect to the position of R, we obtain that those spatial derivatives of u0v ðhÞ have a part which is a measure concentrated on the interface, and consequently u0v ðhÞ ‘‘escapes’’ from the functional space V in which we differentiate. The remedy is simply to rewrite the state Eq. (3.2) as a transmission problem. We thus introduce the restrictions u0 to X0, and u1 to X1, of the solution uv of (3.2). In other words, they satisfy uv = (1 v)u1 + vu0 and are solutions of the transmission problem

8 > divðA1 eðu1 ÞÞ ¼ f 1 > > > > 1 > > < u ¼ uD 1

in X1 ; on C1D ¼ CD \ @ X1 ;

on C1N ¼ CN \ @ X1 ; A eðu Þn ¼ g > > > > u1 ¼ u0 on R ¼ @ X0 \ @ X1 ; > > > : 1 1 1 0 0 0 A eðu Þn þ A eðu Þn ¼ 0 on R 1

1

1

ð3:15Þ

and

8 divðA0 eðu0 ÞÞ ¼ f 0 > > > > 0 > > < u ¼ uD A0 eðu0 Þn0 ¼ g 0 > > > > u0 ¼ u1 > > : 0 0 0 A eðu Þn þ A1 eðu1 Þn1 ¼ 0

in X0 ; on C0D ¼ CD \ @ X0 ; on C0N ¼ CN \ @ X0 ; ;

ð3:16Þ

on R; on R

which is equivalent to (3.2). Recall that n = n0 = n1 denotes the outward unit normal vector to the interface R. Introducing the notations ri(vi) = Aie(vi) and ri(qi) = Aie(qi), the general Lagrangian is deﬁned as

Lðv 1 ; v 0 ; q1 ; q0 ; RÞ ¼

1 1 j ðx; v 1 Þ þ r1 ðv 1 Þ eðv 1 Þ r1 ðv 1 Þ eðq1 Þ þ f 1 q1 dV 2 X1 Z h Z i 1 0 0 þ j ðx; v 0 Þ þ r0 ðv 0 Þ eðv 0 Þ r0 ðv 0 Þ eðq0 Þ þ f 0 q0 dV þ g 0 q0 þ h ðx; v 0 Þ dS 0 0 2 X CN Z Z Z 1 1 1 ½g 1 q1 þ h ðx; v 1 ÞdS ðr1 ðv 1 Þ þ r0 ðv 0 ÞÞn ðq1 q0 ÞdS ðr1 ðq1 Þ þ 2 R 2 R C1N Z 1 ðr1 ðv 1 Þ þ r0 ðv 0 ÞÞn ðv 1 v 0 ÞdS; þ r0 ðq0 ÞÞn ðv 1 v 0 ÞdS þ 2 R

Z

ð3:17Þ

where q0 and q1 play the role of Lagrange multiplier or, at optimality, of the adjoint state p0 and p1(on the same token, at optimality v0, v1 are equal to u0, u1). The functions v0, v1 satisfy non homogeneous Dirichlet boundary conditions and belong to the afﬁne space V, while the other functions q0, q1 vanishes on CD and thus belong to the vector space V0 deﬁned as

G. Allaire et al. / Journal of Computational Physics 230 (2011) 5010–5044

5019

V 0 ¼ fu 2 H1 ðX; Rd Þ such that u ¼ 0 on CD g: Of course, differentiating the Lagrangian with respect to q0 and q1, and equaling it to 0, provides the state Eqs. (3.15) and (3.16). The next result states that differentiating the Lagrangian with respect to v0 and v1, and equaling it to 0, yields the adjoint equation. Lemma 3.3. The optimality condition

@L 1 0 1 0 @L ðu ; u ; p ; p ; vÞ ¼ 0 ðu1 ; u0 ; p1 ; p0 ; vÞ ¼ 0 @v 1 @v for variations in V0 is equivalent to the adjoint problem (3.6). Proof. This is a classical computation [3,26,51] which we do not detail. Differentiating the Lagrangian with respect to v0 and

v1 and equaling it to zero yields

8 0 > divðAi eðpi ÞÞ ¼ ji ðx; ui Þ divðAi eðui ÞÞ > > > > > > > pi ¼ 0 > < 0 i i i i i i i > A eðp Þn ¼ hi ðx; u Þ þ A eðu Þn > > > > > p0 ¼ p1 > > > : 0 0 A eðp Þn ¼ A1 eðp1 Þn

in Xi ; on CiD ; on CiN ;

ð3:18Þ

on R; on R;

which is equivalent to (3.6). h As we already said, the solution uv of (3.2) is not shape differentiable. However its Lagrangian or transported counterpart, namely h ? uv(Id+h) (Id + h), is actually differentiable by a simple application of the implicit function theorem (see Chapter 5 in [38]). As a consequence, upon a suitable extension outside Xi, the solution ui of (3.15) and (3.16) are indeed shape differentiable. Lemma 3.4. The solutions u1 of (3.15) and u0 of (3.16) are shape differentiable. The main interest of the Lagrangian is that its partial derivative with respect to the shape v, evaluated at the state uv and adjoint pv, is equal to the shape derivative of the cost function. Lemma 3.5. The cost function J(v) admits a shape derivative which is given by

J 0 ðvÞðhÞ ¼

@L 1 0 1 0 ðu ; u ; p ; p ; vÞðhÞ; @v

ð3:19Þ

where (u1, u0, p1, p0) are the solutions of the state Eq. (3.15) and (3.16) and adjoint Eq. (3.18). Proof. This is again a classical result [3,26] which we brieﬂy recall. We start from the identity

JðvÞðhÞ ¼ Lðu1 ; u0 ; q1 ; q0 ; vÞ; 1

ð3:20Þ

0

where q , q are any functions in V. We differentiate (3.20) with respect to the shape. By virtue of Lemma 3.4 we obtain

J 0 ðvÞðhÞ ¼

@L 1 0 1 0 @L @u0;1 1 0 1 0 ðu ; u ; q ; q ; vÞðhÞ þ ðu ; u ; q ; q ; v Þ; ðhÞ : @v @ v 0;1 @v

ð3:21Þ

The notation @L means that it is a shape partial derivative, i.e., we differentiate L in the sense of Deﬁnition 3.1 while keeping @v the other arguments (u1, u0, q1, q0) ﬁxed. Taking now (q1, q0) = (p1, p0) cancels the last term in (3.21) because it is the variational formulation of the adjoint problem by virtue of Lemma 3.3. We thus obtain (3.19). h To ﬁnish the proof of Theorem 3.1 it remains to compute the partial shape derivative of the Lagrangian. It is a conceptually simple application of Lemma 3.1 which, nevertheless, is quite tedious. Therefore the proof of the following Lemma is postponed to Appendix A. Lemma 3.6. The partial shape derivative of the Lagrangian

@L 1 0 1 0 ðu ; u ; p ; p ; vÞðhÞ; @v is precisely equal to the right hand side of (3.9).

5020

G. Allaire et al. / Journal of Computational Physics 230 (2011) 5010–5044

4. Topological derivative The aim of this section is to evaluate the sensitivity of the cost function to the introduction of an inﬁnitesimal damaged region xq inside the healthy region X1. In theory the shape of the smooth inclusion can be arbitrary. However, for practical and numerical purposes it will be assumed to be a ball in Rd . 4.1. Main result Let x be a smooth open subset of Rd . Let q > 0 be a small positive parameter which is intended to go to zero. For a point x0 2 X1 we deﬁne a rescaled inclusion

xq ¼ x 2 Rd :

x x0

q

2x ;

ð4:1Þ

which, for small enough q is strictly included in X1 and disconnected from X0. The total damaged zone is thus X0q :¼ X0 [ xq and the healthy phase is X1q :¼ X n X0q . Let vq ; v; vxq denote the characteristic functions of X0q ; X0 and xq, respectively (ver0 ifying vq ¼ v þ vxq ). In the sequel, in order to distinguish integration in the variables x and y :¼ xx q , the symbol dV will sometimes be replaced by dV(y) or dV(g) (where g is a dummy variable similar to y). Let us recall the notations for the non-perturbed domain X = X0 [ X1 (i.e., without the damage inclusion). The cost function then writes as

JðvÞ ¼

1 2

Z

Av eðuv Þ eðuv ÞdV þ

Z

X

X

jv ðx; uv ÞdV þ

Z

hv ðx; uv ÞdS;

ð4:2Þ

@X

where jv = j0v + j1(1 v), hv = h0v + h1(1 v), and the so-called ‘‘background’’ solution’’ uv solves the state Eq. (3.2) on X = X0 [ X1. As in the previous section, we assume that the integrands j0, j1(x, u) and h0, h1(x, u) are twice differentiable functions with respect to u, satisfying the growth conditions (3.4). Moreover, let us recall that the so-called ‘‘background’’ dual solution pv solves the adjoint problem (3.6) on X = X0 [ X1. On the perturbed domain X ¼ X0q [ X1q , the cost function is

Jðvq Þ ¼

1 2

Z

X

Avq eðuvq Þ eðuvq ÞdV þ

Z

X

jvq ðx; uvq ÞdV þ

Z

@X

hv ðx; uvq ÞdS;

because vq v, and thus hvq hv , on @ X (the inclusion xq is away from the boundary), and where uvq solves

8 divðAvq eðuvq ÞÞ ¼ f > > < uvq ¼ uD > > : A eðu Þn ¼ g vq

vq

in X; on CD ;

ð4:3Þ

on CN ;

with Avq ¼ A0 vq þ A1 ð1 vq Þ, the Lamé tensor of the material with the inclusion. Deﬁnition 4.1. If the objective function admits the following so-called topological asymptotic expansion for small q > 0:

Jðvq Þ JðvÞ qd DJðx0 Þ ¼ oðqd Þ then the number DJ(x0) is called the topological derivative of J at x0 for the inclusion shape x. The main result of this section is the following theorem. Theorem 4.1. The topological derivative DJ(x0) of the general cost function (4.2), evaluated at x0 for an inclusion shape x, has the following expression:

1 0 1 DJðx0 Þ :¼ Meðuv Þðx0 Þ eðpv Þðx0 Þ Meðuv Þðx0 Þ eðuv Þðx0 Þ þ jxjðj j Þðx0 ; uv ðx0 ÞÞ; 2

ð4:4Þ

where uv and pv are the solution to the primal and dual problems (3.2) and (3.6), respectively, and where M is the so-called elastic moment tensor as deﬁned below by (4.10). Moreover, M is positive if [A] is positive, and negative if [A] is negative. In the case of our damage model, the cost function is (2.4), i.e., jv(x, uv) = jv f uv and hv(x, uv) = g uv. The problem is then known to be self-adjoint, i.e., the adjoint pv is equal to 0. In such a case Theorem 4.1 simpliﬁes as follows. Corollary 4.1. The topological derivative of the cost function (2.4) at x0 for an inclusion shape x is

1 DJðx0 Þ :¼ jxjj Meðuv Þðx0 Þ eðuv Þðx0 Þ; ; 2 where uv is the background solution of (3.2) and M is the elastic moment tensor deﬁned below by (4.10).

ð4:5Þ

5021

G. Allaire et al. / Journal of Computational Physics 230 (2011) 5010–5044

In 2d, the elastic moment tensor M for a unit disk-inclusion x has been computed in [10]. The topological derivative (4.5) for a disk-inclusion is:

l1 ½lðk1 þ 2l1 Þ DJðx0 Þ ¼ pj 2p eðuv Þ eðuv Þðx0 Þ k1 ðl0 þ l1 Þ þ l1 ðl1 þ 3l0 Þ p ðk1 þ 2l1 Þ½k þ l l1 ½lðk1 þ 2l1 Þ þ þ2 treðuv Þtreðuv Þðx0 Þ: k0 þ l0 þ l1 k1 ðl0 þ l1 Þ þ l1 ðl1 þ 3l0 Þ 2 In 3d, the elastic moment tensor M for a unit ball-inclusion x has also been computed in [11]. The topological derivative (4.5) for a ball-inclusion is:

DJðx0 Þ ¼ with

4p 2p ½kb 2½la j treðuÞtreðuÞ ; 2½leðuÞ eðuÞ þ ð3a þ bÞ 3 3b

m1 ¼ 2ðk1kþ1 l1 Þ and a :¼

5l1 m1 ½k k1 ½l ; 15k1 l1 ð1 m1 Þ

b :¼

15l1 ð1 m1 Þ 2½lð4 5m1 Þ > 0: 15l1 ð1 m1 Þ

In order to prove Theorem 4.1 we need several technical tools detailed in the next subsections. 4.2. Elastic moment tensor The goal of this subsection is to deﬁne the elastic moment tensor as a 4th order tensor expressing the leading behavior in the far ﬁeld of wn, solution to the canonical problem (4.9) of a unit damage inclusion x in a uniform healthy background. 0 We introduce a microscopic variable y ¼ xx q in order to rescale the problem with a unit inclusion x. This rescaling, centered on the inclusion, in the limit as q goes to zero, transforms the elasticity problem posed on X in a problem posed on Rd . The symbols ey, divy etc. are used to specify the derivation w.r.t. y. We begin by recalling the Green tensor for linear elasticity in a uniform inﬁnite material. Notation 4.1 (Green tensor of elasticity). The fundamental tensor of linear elasticity C :¼ (Cij)16i,

Cij ðyÞ :¼

8 < 4ap

yy 4bp jyji dj jyjd2 : a dij ln jyj b yi y2j 2p jyj 2p dij

j6d

reads:

if d P 3; if d ¼ 2;

ð4:6Þ

;

where

a¼

1 2

1

1

þ 1

! and b ¼

1 2

1

1

1

!

: l 2l1 k1 2l1 þ k1 The component Cij represents the ith Cartesian component of the fundamental solution in the free-space with a unit Dirac

l

load d0 at the origin in the direction of vector ej, that is, 1

div A ey

d X

!!

Cij ei

¼ ej d0 ;

ð4:7Þ

i¼1

where ek denotes the kth element of the canonical basis of Rd . We introduce the following Hilbert space (so-called Deny-Lions or Beppo-Levi space)

W :¼ fw 2 H1loc ðRd ; Rd Þ such that eðwÞ 2 L2 ðRd ; Rdd Þg; 2

ð4:8Þ

d

equipped with the scalar product of L ðR Þ for the deformation tensor e(w), which is well adapted to elasticity problems posed in the whole space Rd . For any symmetric matrix n we introduce wn(y), solution to the canonical problem

(

divy ðAvx ey ðwn ÞÞ ¼ divy ðvx ½AnÞ in Rd ; wn 2 W;

ð4:9Þ

which is easily seen to be well-posed. The fact that wn belongs to W implies it has some decay properties at inﬁnity (by embedding of W in some Lebesgue space, see [29,2]). We shall not dwell on them since Lemma 4.1 below improve these decay properties. Lemma 4.1 (Far ﬁeld expression). The solution wn of the canonical problem (4.9) has the following pointwise behavior at inﬁnity:

wn ¼ @ p Cq ðyÞM pqkl nkl þ Oðjyjd Þ as jyj ! 1;

ð4:10Þ

5022

G. Allaire et al. / Journal of Computational Physics 230 (2011) 5010–5044

where Cq :¼ Ckqek is the fundamental Green’s tensor of linear elasticity of the healthy material, and M is the 4th order elastic moment tensor with respect to inclusion x, independent of n, deﬁned by

M ¼ ½AðN þ jxjI4 Þ

ð4:11Þ

with a 4th order tensor N deﬁned by

Nn :¼

Z

ey ðwn ÞdVðyÞ::

ð4:12Þ

x

Remark 4.1. Lemma 4.1 tells us that, because the right hand side in (4.9) has zero average, wn behaves like Oðjyjdþ1 Þ at inﬁnity. The interest of the canonical problem for us is that, by denoting n0 = e(uv)(x0), we shall prove in some sense

x x0 :

uvq ðxÞ uv ðxÞ þ qwn0

q

Remark 4.2. The elastic moment tensor M as deﬁned by (4.11) is exactly the same tensor as introduced in [8,10] (by means of layer potential techniques) or in [25] (by means of a variational approach in the conductivity setting). Proof of Lemma 4.1. Let us consider an inclusion x located in the free-space Rd and introduce a smooth open set U strictly containing x and a cut-off function u 2 C 1 ðRd Þ such that u 0 on x, u 1 on Rd n U. We deﬁne a function f(y) by

f :¼ divy Avx eðuwn Þ ;

ð4:13Þ d

which has compact support in U because of (4.9) and the fact that u 1 on R n U. Since u 0 on x we deduce that

(

divy ðA1 ey ðuwn ÞÞ ¼ f

in Rd ;

ð4:14Þ

uwn 2 W: We can thus use the Green tensor to compute the kth component of the solution of (4.14)

uðyÞek wn ðyÞ ¼

Z

Ckq ðy gÞfq ðgÞdVðgÞ:

Rd

ð4:15Þ

It turns out that

Z

Z Z Z ð4:9Þ f ðyÞdVðyÞ ¼ Avx eðuwn ÞndSðyÞ ¼ divðAvx eðwn ÞÞdVðyÞ ¼ divðvx ½AnÞdVðyÞ U @U U U Z ¼ vx ½Ann dSðyÞ ¼ 0

f ðyÞdVðyÞ ¼

Rd

Z

@U

with n denoting the usual normal unit vector to @U. By Taylor expansion of the Green function Ckq(y g) in terms of Ckq(y) and its derivatives, taking into account that f has zero average and compact support in U, and since u 1 away from U, (4.15) yields that

ek wn ðyÞ ¼ @ p Ckq ðyÞ

Z Rd

gp fq ðgÞg þ Oðjyjd Þ:

ð4:16Þ

R

Let us now evaluate Rd gp fq ðgÞdVðgÞ that for the sake of calculus is rewritten as second order tensor. By (4.13) and since A1 ¼ Avx on @U,

Z

U

R

Rd

Bpq g f ðgÞdVðgÞ, where Bpq :¼ eq ep is a

Z Avx eðuwn Þ eðBpq gÞdVðgÞ Avx eðuwn Þn Bpq gdSðgÞ U @U Z Z A1 eðuwn Þ eðBpq gÞdVðgÞ A1 eðuwn Þn Bpq gdSðgÞ ¼ U @U Z Z Z divðA1 eðBpq gÞÞ uwn dVðgÞ þ A1 eðBpq gÞn uwn dSðgÞ A1 eðuwn Þn Bpq gdSðgÞ ¼ U |ﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄ{zﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄ} @U @U

Bpq g f ðgÞdVðgÞ ¼

Z

¼0

Z

ðAvx eðB gÞn wn Avx eðwn Þn Bpq gÞdSðgÞ Z Z

divðAvx eðBpq gÞÞ wn dVðgÞ div Avx eðwn Þ Bpq gdVðgÞ ¼ U |ﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄ{zﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄ} U |ﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄ{zﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄ} ¼

pq

@U

¼

Z x

¼divðvx ½ABpq Þ pq

½AB eðwn ÞdVðgÞ þ

Z x

¼divðvx ½AnÞ

pq

½An B dVðgÞ ¼ ½ABpq

Z x

ðeðwn Þ þ nÞdVðgÞ:

ð4:17Þ

G. Allaire et al. / Journal of Computational Physics 230 (2011) 5010–5044

5023

Introducing Mijkl deﬁned as

Mijkl :¼ ½Aijmn ðN þ jxjI4 Þmnkl

ð4:18Þ

we obtain (4.10). h Lemma 4.2 (Symmetry and signature of M). The elastic moment tensor M, deﬁned by (4.11), is symmetric and positive if A0 < A1 while negative if A0 > A1. Proof of Lemma 4.2. Let us multiply (4.9) by the solution wn0 for another symmetric tensor n0 , integrate by parts and observe that, by the symmetry property of the left hand side, we have

Z Rd

Avx eðwn Þ eðwn0 ÞdV ¼ ½An Nn0 ¼ ½An0 Nn ¼ ½AN n n0 ¼ ½AN n0 n;

ð4:19Þ

the symmetry of [A]N and hence of M immediately follows. Take n = n0 in (4.19), then [A]N is clearly positive. Therefore if [A] > 0, then M is obviously positive. Assume now that [A] < 0. The solution wn of (4.9) is the minimizer of the following energy

IðwÞ ¼

1 2

Z Rd

Avx eðwÞ eðwÞdV

Z Rd

vx ½An eðwÞdV

and its minimal value is, by (4.12), Iðwn Þ ¼ 12 ½ANn n. On the other hand as soon as we rewrite

Avx eðwÞ eðwÞ ¼ vx ½AeðwÞ eðwÞ þ A1 eðwÞ eðwÞ we obtain the lower bound I(w):

IðwÞ P I ðwÞ :¼

1 2

Z Rd

vx ½AeðwÞ eðwÞdV

Z Rd

vx ½An eðwÞdV:

It is easily seen that e(w) = n is a critical point in x of the above lower bound, which, by the negative character of [A], turns out to be the unique minimizer, thereby providing the minimal value 12 jxj½An n. Thus we deduce that

jxj½An n 6 ½ANn n which implies the desired result M < 0.

h

4.3. Asymptotic analysis in the perturbed domain This subsection is aimed at comparing the solutions of elasticity problems in the perturbed and non-perturbed domains. We deﬁne the difference v :¼ uvq uv between the perturbed (uvq ) and the background (uv) displacement ﬁelds. The equation satisﬁed by v is

8 divðAvq eðv ÞÞ ¼ divðvxq ½Aeðuv ÞÞ in X; > > > < v¼0 on CD ; > > > : A eðv Þn ¼ 0 on CN : vq

ð4:20Þ

Let us introduce atensor n0 :¼ e(uv)(x0) and let wn0 ðyÞ be the solution of (4.9) for n = n0. We deﬁne a rescaled function 0 which is a solution to wqn0 ðxÞ :¼ qwn0 xx q

¼ div ½Avxq eðuv Þðx0 Þ in X; div Avq e wqn0

satisfying non-homogeneous, but small, boundary conditions. This function wqn0 is the leading term of a so-called inner asymptotic expansion for v as stated by the following Lemma. Lemma 4.3. For any cut-off function h 2 C 1 c ðXÞ such that h 1 in a neighborhood U of x0, there exists a constant C > 0 independent of q such that we have

v ¼ hwqn

0

þ d;

ð4:21Þ

with

kdkH1 ðXÞ 6 C qd=2þ1 :

ð4:22Þ

5024

G. Allaire et al. / Journal of Computational Physics 230 (2011) 5010–5044

Moreover

( q

kwn0 kL2 ðXÞ 6 C

pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ

q2 log q if d ¼ 2 and keðwqn0 ÞkL2 ðXÞ 6 C qd=2 : qd=2þ1 if d P 3

ð4:23Þ

Remark 4.3. In the vicinity of the inclusion xq, we have h 1 for sufﬁciently small q, and (4.21) can be restated as

v ðxÞ ¼ qwn

x x0

q

0

þ oH1 ðqÞ;

which is an inner asymptotic expansion for v, solution of (4.20). The L2-norms of d and wqn0 are of the same order (at least for d P 3) but the L2-norm of rd is smaller by a factor q than that of rwqn0 , which explains the o(q) remainder in the above approximation of v. Proof of Lemma 4.3. The estimates (4.23) on wqn0 are simply obtained by rescaling and by the decay properties of wn0 . We obtain

keðwqn0 Þk2L2 ðXÞ ¼

Z

jey ðwn0 Þ

X

Z x 2 j dV ¼ qd

q

X=q

jey ðwn0 ÞðyÞj2 dVðyÞ 6 C qd :

Similarly

kwqn0 k2L2 ðXÞ ¼ q2

Z X

jwn0

Z x 2 j dV ¼ qdþ2

q

X=q

jwn0 ðyÞj2 dVðyÞ:

However, Lemma 4.1 tells us that the behavior at inﬁnity of wn0 is such that it does not belong to L2 ðRd Þ but is of the order of Oðjyjdþ1 Þ. Therefore, using the radial coordinate r = jyj yields q

kwn0 k2L2 ðXÞ

6 Cq

dþ2

Z X=q

1 1 þ jyj

dVðyÞ 6 C q 2ðd1Þ

dþ2

Z 1

1=q

dr 6C r d1

(

q4 j log qj if d ¼ 2; qdþ2 if d P 3

ð4:24Þ

which is the desired result. Furthermore, since wn0 ¼ Oðjyjdþ1 Þ and rwn0 ¼ Oðjyjd Þ at inﬁnity, we also deduce by rescaling that

kwqn0 kL1 ðXnUÞ 6 C qd and krwqn0 kL1 ðXnUÞ 6 C qd :

ð4:25Þ

We now write the equation satisﬁed by d:

8 > > < divðAvq eðdÞÞ ¼ div ½Avxq ðeðuv ÞðxÞ eðuv Þðx0 ÞÞ þ g d¼0 > > : Avq eðdÞn ¼ 0

in X; ð4:26Þ

on CD ; on CN ;

where

g ¼ div½Avq eðhwqn0 Þ hdiv½vxq ½Aeðuv Þðx0 Þ:

ð4:27Þ

Let us multiply (4.26) and (4.27) by d and integrate by parts, in such a way that

Z Z CkeðdÞk2L2 ðXÞ 6 Avq eðdÞ eðdÞdV 6 X

xq

Z ½Aðeðuv ÞðxÞ eðuv Þðx0 ÞÞ eðdÞdV þ g ddV :

ð4:28Þ

X

for C > 0. Let us remark that, away from the interface between the two phases, uv is of class C 2;a for some a > 0 (since we assume the forces to be of class C 0;a ). Furthermore, the inclusion xq is smooth, so the C 2;a regularity of uv holds up to the interface in the inclusion, and hence

jeðuv ÞðxÞ eðuv Þðx0 Þj 6 C q in xq ;

ð4:29Þ

which implies

Z xq

½Aðeðuv ÞðxÞ eðuv Þðx0 ÞÞ eðdÞdV 6 C qd=2þ1 keðdÞk 2 : L ðXÞ

ð4:30Þ

Moreover by (4.27), it results that

Z Z Z Z g ddV ¼ Avq eðhwqn0 Þ eðdÞdV þ vxq ½Aeðuv Þðx0 Þ eðhdÞdV ¼ Avq eðhwqn0 Þ eðdÞdV þ Avq eðwqn0 Þ eðhdÞdV X X X X Z X q s q s Avq eðwn0 Þ ðd rhÞ eðdÞ ðwn0 rhÞ dV; ¼ ð4:31Þ

Z

X

G. Allaire et al. / Journal of Computational Physics 230 (2011) 5010–5044

5025

where the superscript ‘‘s’’ stands for the symmetric part. Hence, since rh vanishes on a neighborhood U of xq, by Korn inequality and by estimates (4.25), it follows that

Z q d g ddV 6 C kwq k 1 n0 L ðXnUÞ þ keðwn0 ÞkL1 ðXnUÞ krhkL2 ðXnUÞ keðdÞkL2 ðXÞ 6 C q keðdÞkL2 ðXÞ :

ð4:32Þ

X

Therefore, by (4.28)–(4.32) and since d/2 + 1 6 d for d P 2, the following global estimate holds

keðdÞkL2 ðXÞ 6 C qd þ qd=2þ1 6 C qd=2þ1 ;

ð4:33Þ

completing the proof by Korn and Poincaré inequalities. h Similarly, we shall need a comparison between the perturbed and background adjoints. However, the adjoint in the perturbed domain (with an inclusion) is not the standard one. Rather, we introduce a slightly different adjoint problem

8 ~vq ÞÞ ¼ fv þ j0v ðx; uv Þ in X; > divðAvq eðp > < ~ vq ¼ 0 on CD ; p > > 0 : A eðp on CN ; vq ~ vq Þn ¼ g v þ hv ðx; uv Þ

ð4:34Þ

~vq depends on the inclusion since the Lamé tensor Avq corresponds to the perturbed domain X ¼ X0q [ X1q . whose solution p ~vq is different from pv , deﬁned by (3.6) with vq instead of v, because the right hand side of (4.34) depends Nevertheless, p q only on v and not on vq. ~vq pv , which is We deﬁne the difference between the above perturbed adjoint and the ‘‘true’’ background adjoint, q :¼ p the solution of

8 divðAvq eðqÞÞ ¼ divðvxq ½Aeðpv ÞÞ in X; > < q¼0 on CD ; > : Avq eðqÞn ¼ 0 on CN :

ð4:35Þ

We introduce the tensor n00 :¼ eðpv Þðx0 Þ and the rescaled function wqn0 ðxÞ :¼ qwn00 0

xx0

q

which is the leading term of an inner

asymptotic expansion for q. Lemma 4.3 can then be generalized as follows. Lemma 4.4. For any cut-off function h 2 C 1 c ðXÞ such that h 1 in a neighborhood U of x0, there exists a constant C > 0 independent of q such that we have

q ¼ hwqn0 þ d; 0

with

kdkH1 ðXÞ 6 C q1þd=2 ::

ð4:36Þ

Moreover

(

pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ

q2 log q if d ¼ 2 and keðwqn0 ÞkL2 ðXÞ 6 C qd=2 : kwn0 kL2 ðXÞ 6 C 0 0 qd=2þ1 if d P 3 q

4.4. Proof of Theorem 4.1 We combine the ingredients of the two previous subsections to prove Theorem 4.1 on the topological derivative. Let us recall that we assume the integrands of the objective function, j0, j1(x, u) and h0, h1(x, u), to be C2 functions with respect to u with adequate growth conditions. Recalling that hvq hv on @ X because the inclusion does not touch the boundary, we write a second-order Taylor expansion of the objective function

Jðvq Þ ¼

1 2

Z

þ

Av eðuv þ v Þ eðuv þ v ÞdV

X

Z

hv ðuv þ v ÞdS þ @X

xq

0

Z xq

½Aeðuv þ v Þ eðuv þ v ÞdV þ

1

ðj j Þðuv þ v ÞdV ¼ JðvÞ þ

Z X

Z X

jv ðuv þ v ÞdV

Av eðuv Þ eðv ÞdV þ

1 2

Z

Av eðv Þ eðv ÞdV

X

Z Z Z 1 0 0 ½Aeðv Þ eðv ÞdV þ jv ðx;uv Þ v dV þ hv ðx; uv Þ v dS 2 xq xq X @X Z Z Z Z 1 1 1 00 0 1 00 0 1 0 1 ðj j Þðuv ÞdV þ jv ðuv Þv v dV þ hv ðuv Þv v dS þ ðj j Þ0 ðuv Þ v dV þ ðj j Þ00 ðuv Þv v dV; þ 2 X 2 @X 2 xq xq xq

1 2 Z

Z

Z

1 2

½Aðeðuv Þ eðuv Þ þ 2eðuv Þ eðv ÞÞdV

ð4:37Þ

5026

G. Allaire et al. / Journal of Computational Physics 230 (2011) 5010–5044 00

00

where uv ¼ uv þ fv with 0 < f < 1. From assumption (3.4) we know that jv and hv are bounded on X and thus

Z j00 ðuv Þv v dV 6 Ckv k22 6 oðqd Þ v L ðXÞ X

and, since

Z

@X

v = d on @ X,

Z 00 hv ðuv Þv v dS ¼

@X

00 hv ðuv Þd d dS 6 Ckdk2H1 ðXÞ 6 oðqd Þ

by Lemma 4.3. A similar estimate holds for the last term of (4.37). The penultimate term is bounded by

Z 0 1 0 ðj j Þ ðuv Þ v dV 6 C qd=2 kuv kL1 ðxq Þ þ 1 kv kL2 ðXÞ 6 oðqd Þ xq because the background solution uv is smooth on xq (it does not ‘‘see’’ the inclusion). Thus, the two last lines of (4.37) are small of the order of o(qd). All other terms in (4.37) contribute to the ﬁnal result, formula (4.4). First, by rescaling and continuity of uv on xq, we have

Z

0

1

0

1

ðj j Þðuv ÞdV ¼ qd jxjðj j Þðuv ðx0 ÞÞ þ oðqd Þ:

xq

Similarly, by continuity of e(uv), using the notation n0 = e(uv)(x0), and since

1 2

Z xq

½Aðeðuv Þ eðuv Þ þ 2eðuv Þ eðv ÞÞd ¼

d

q

Z

2

x

v ¼ hwqn

0

½Aðn0 n0 þ 2n0 ey ðwn0 ÞÞdVðyÞ þ

þ d with h 1 in xq, we deduce

Z

½Aeðuv Þ eðdÞdV þ oðqd Þ: xq

Using again the continuity of e(uv) in xq and (4.36), we bound the last term

j

Z

½Aeðuv Þ eðdÞdVj 6 C qdþ1 :

xq

Second, from the variational formulation of (4.20) we get

1 2

Z

Av eðv Þ eðv ÞdV X

1 2

Z xq

½Aeðuv ðv Þ eðv ÞdV ¼ ¼

where we have again replaced

Z

Av eðuv Þ eðv Þ dV ¼

Z

X

v by wqn

0

Z

qd

Avq eðv Þ eðv ÞdV ¼

X

Z

2

x

1 2

Z xq

½Aeðuv Þ eðv ÞdV

½An0 ey ðwn0 ÞdVðyÞ þ oðqd Þ;

þ d in xq and neglected the d term. Third, from (3.2) we have

fv v dV þ

X

1 2

Z

@X

g v v dS:

Thus, the Taylor expansion (4.37) of the objective function is rewritten

Jðvq Þ ¼ JðvÞ þ

Z Z 0 fv þ jv ðx; uv Þ v dV þ

Z qd 0 g v þ hv ðx; uv Þ v dS ½Aðn0 n0 þ n0 ey ðwn0 ÞÞdVðyÞ 2 x @X

X

0

1

þ qd jxjðj j Þðuv ðx0 ÞÞ þ oðqd Þ:

ð4:38Þ

By Lemma 4.1 we know that

qd 2

Z x

½Aðn0 n0 þ n0 ey ðwn0 ÞÞdVðyÞ ¼

qd 2

Mn0 n0 :

It remains to show that the two ﬁrst integrals in the right hand side of (4.38) are of order Oðqd Þ and ﬁnd formula (4.4) for the topological derivative. To do so, we use the adjoint problems (4.34) and (4.35) as follows. Multiplying (4.34) by v and (4.20) ~vq we obtain by p

Z Z Z Z 0 0 ~vq Þ eðv ÞdV ¼ fv þ jv ðx; uv Þ v dV þ ðg v þ hv ðx; uv ÞÞ v dS ¼ Avq eðp X

@X

¼

Z

xq

X

xq

¼ qd

½Aeðuv Þ eðpv þ qÞdV ¼

Z x

~vq ÞdV ½Aeðuv Þ eðp Z xq

½Aeðuv Þ eðpv þ hwqn0 þ dÞdV 0

½An0 n00 þ ey ðwn00 Þ dVðyÞ þ oðqd Þ ¼ qd Mn0 n00 þ oðqd Þ;

by application of Lemma 4.4, rescaling, using the continuity of e(uv) and e(pv) in xq and thanks to the formula for M in Lemma 4.1 (recall that n00 ¼ eðpv Þðx0 Þ). Eventually we have proved

G. Allaire et al. / Journal of Computational Physics 230 (2011) 5010–5044

Jðvq Þ ¼ JðvÞ

qd 2

0

5027

1

Mn0 n0 þ qd Mn0 n00 þ qd jxjðj j Þðuv ðx0 ÞÞ þ oðqd Þ;

which is precisely formula (4.4). This achieves the proof of Theorem 4.1 since the properties of M have been proved in Lemma 4.2. 5. Computational algorithm The main task is to compute, for each discrete time ti, i P 0, a minimizer vi of the Francfort–Marigo model (2.8). As we already said, we are interested in local minima. Our notion of local minima is numerical in essence, that is, we minimize (2.8) with a gradient descent algorithm in the level set framework. A minimum is thus local in the sense of perturbations of the location of the interface R. Our algorithm is made of two nested loops: (i) An outer loop corresponding to the increasing sequence of discrete times ti, i P 0. (ii) An inner loop of gradient iterations for the minimization of the functional (2.8) at each ﬁxed time step ti. The irreversibility constraint (2.7) on the damaged zone is taken into account in the outer loop (i), whereas the inner loop (ii) is purely numerical and is not subject to this irreversibility constraint between two successive iterates of (ii). The inner loop is performed with the level set method of Osher and Sethian [50] that we now brieﬂy describe (it is very similar with its application in the context of shape optimization [5,62]). In the ﬁxed bounded domain X, uniformly meshed once and for all, we parametrize the damaged zone X0 by means of a level set function w such that

8 > < wðxÞ ¼ 0 () x 2 R; wðxÞ < 0 () x 2 X0 ; > : wðxÞ > 0 () x 2 X1 : The normal n to the damaged region X0 is recovered as rw/jrwj and the mean curvature H is given by the divergence of the normal div n. These quantities are evaluated by ﬁnite differences since our mesh is uniformly rectangular. Although n and H are theoretically deﬁned only on R, the level-set method allows to deﬁne easily their extension in the whole domain X. Following the minimization process, the damaged zone is going to evolve according to a ﬁctitious time s which corresponds to descent stepping and has nothing to do with the ‘‘real’’ time ti in the outer loop (i). As is well-known, if the shape is moving with a normal velocity V, then the evolution of the level-set function is governed by a simple Hamilton–Jacobi equation [49,57],

@w þ Vjrwj ¼ 0; @s

ð5:1Þ

which is posed in the whole body X, and not only on the interface R, when the velocity V is known everywhere. We now explain how we derive V for our speciﬁc problem. For the minimization of (2.8) we use the shape derivative given by (3.9),

J 0 ðvÞðhÞ ¼

Z

Dh n dS;

ð5:2Þ

R

where the integrand DðxÞ 2 L2 ðRÞ is given by Theorem 3.1 and h 2 W 1;1 ðX; Rd Þ in any admissible direction of derivation. Since only the normal component of h plays a role in (5.2), we always look for a normal vector ﬁeld, i.e., we restrict our attention to

h ¼ v n with a scalar field

v 2 W 1;1 ðXÞ:

ð5:3Þ

The velocity V is going to be chosen as an ‘‘optimal’’ direction of derivation, v, such that

J 0 ðvÞðV nÞ ¼

Z

DV dS 6 0:

ð5:4Þ

R

The simplest choice V ¼ D, which enforces (5.4) and is commonly used in structural optimization [5], is not satisfactory in the present situation, since D is deﬁned as a jump on R only, without natural extension over X. We therefore suggest another choice based on the identiﬁcation of the duality product between J0 (v) and v (recalling that h = v n) with the usual scalar product in H1(X). In other words we represent J0 (v) by a scalar ﬁeld ðVÞ 2 H1 ðXÞ such that, for any test function v,

J 0 ðvÞðv nÞ ¼

Z

ðrV rv þ V v ÞdV:

ð5:5Þ

X

Combining (5.2) and (5.5), and requiring the descent condition (5.4), we choose the velocity V in (5.1) as the unique solution in H1(X) of the variational formulation

5028

G. Allaire et al. / Journal of Computational Physics 230 (2011) 5010–5044

Z

ðrV rv þ V v Þ dV ¼

Z

Dv dS 8

v 2 H1 ðXÞ:

ð5:6Þ

R

X

Solving (5.6) to compute a shape derivative is a usual trick in shape optimization for regularizing derivatives [3,52]. However, (5.6) is used here mostly for extending the ‘‘natural’’ velocity D away from the interface R. In practice we add a small positive coefﬁcient (linked to the mesh size) in front of the gradient term in (5.6) in order to limit the regularization and the spreading of the velocity around the interface. For numerical purpose, as explained in [5], the surface integral in the right hand side of (5.6) is written as a volume integral

Z

Dv dS ¼

Z

R

dR Dv dV;

ð5:7Þ

X

where the Dirac mass function dR is approximated by

dR ¼

1 jrðs ðwÞÞj 2

with the following approximation of the sign function

wðxÞ s ðxÞ ¼ qﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ; wðxÞ2 þ 2 where > 0 is a small parameter chosen in order to spread the integration over a few mesh cells around the interface. The integrand D, being actually a jump ½E of a discontinuous quantity E (see formulae (3.11) or (3.12)), requires also some special care. In (5.7) we replace D ¼ ½E by

Dapprox ¼ ½Eapprox ¼ 2ðð1 vÞE vEÞ; where v is the characteristic function of the damaged phase (numerically it is always equal to 0 or 1 except in those cells cut by the interface where it is interpolated by the local proportion of damaged phase in the cell). The factor 2 in the above formula takes into account the fact that

Z X

dR v dV

1 2

Z

dS:

R

In our numerical experiments we use formula (3.11) and not (3.10) because the latter one exhibits singular jumps when the damaged phase is very weak (which is the case for our simulations of crack propagation). Of course, in the case of a degenerate (zero) damaged phase we can use the limit formula given by Remark 3.2 which are of course much simpler (we did so in our previous publication [6]). Remark 5.1. Note that the same problem of computing a jump of a discontinuous quantity at an interface was independently addressed in [42]. This work is also relying on the level set method and is applied to the Mumford–Shah functional in image segmentation. It can also be applied to fracture mechanics and, as our proposed approach, it relies on a fattening of the fracture path. Our proposed algorithm for the inner loop (ii) is an iterative method, structured as follows: 1. Initialization of the level set function w0 as the signed distance to the previous damaged interface Ri corresponding to the characteristic function v0 vi. 2. Iteration until convergence, for k P 0: (a) Computation of the state uk by solving a problem of linear elasticity with coefﬁcients Avk ¼ ð1 vk ÞA1 þ vk A0 . (b) Deformation of the interface by solving the transport Hamilton–Jacobi equation (5.1). The new interface Rk+1 is characterized by the characteristic function vk+1 or the level-set function wk+1 solution of (5.1) after a pseudo-time step

Dsk starting from the initial condition wk(x) with velocity V k computed through (5.6) in terms of uk. The pseudo-time step Dsk is chosen such that J(vk+1) 6 J(vk). (c) Irreversibility constraint: we replace vk+1 by max (vk+1, v0) where v0 vi corresponds to the damaged zone at the previous iteration of the outer loop (i). At each iteration of above the inner loop, for stability reasons, we also reinitialize the level-set function w [49,57]. This is crucial because the integrand D of the shape derivative involves normal and tangential components of stress or strain tensors, which requires a precise evaluation of the normal n by formula rw/jrwj. Actually it turns out that this reinitialization step must be much more precise in the present context than for shape optimization [5]. Indeed, a poor reinitialization can inﬂuence the propagation of the damage zone. We therefore use a trick suggested in [54] for an increased accuracy of the second-order reinitialization process. The Hamilton–Jacobi equation (5.1) is solved by an explicit second order upwind scheme on a Cartesian grid. The boundary conditions for w are of Neumann type. Since this scheme is explicit in time, its

G. Allaire et al. / Journal of Computational Physics 230 (2011) 5010–5044

5029

time step is given by a CFL condition. In numerical practice we often take the descent step Dsk of the order of the Hamilton– Jacobi time step which stabilizes the damage evolution. 6. Simulation results Otherwise explicitly mentioned, all our numerical experiments are performed with a healthy material having Young modulus E1 = 1000 and Poisson ratio m1 = 0.3 (white material on the pictures). The damaged phase (black material on the pictures) has always Poisson ratio m0 = 0.3 (the fact that m0 = m1 does not matter) but has different Young modulus in different places. More precisely, in Section 6.1 we consider a moderately weak damaged phase with E0 = 500, while in the next subsections the damage phase is assumed to be almost degenerate, i.e. E0 = 103: this last case corresponds to a limit where our model behaves almost like a brittle fracture model. Actually some models of fracture mechanics [33] are approximated by Cconvergence techniques [20,21], which is similar in spirit to a damage model. Therefore it is not surprising that our damage model can predict crack propagation. In the sequel we call critical load the value of the applied displacement for which the damage region has completely crossed the computational domain (meaning failure of the structure), and initiation load the ﬁrst value for which the damage zone departs from its initialization. All other intermediate load values are called subcritical, while values above the critical one are called supercritical. In order to validate our method, two types of numerical experiments are done. On the one hand, for simple problems we check convergence under various reﬁnements of the mesh size, of the time step, etc. On the other hand, we compare our results with a variety of existing benchmarks tested by laboratory experiments or other numerical methods. 6.1. 2d damage simulation The numerical experiments with a moderately weak damaged phase, E0 = 500, are easier to perform that the ones with a degenerate phase but their results are mechanically less interesting. Therefore we content ourselves with a single experiment, namely a mode I traction (Fig. 1) in a square box of size 1 with a Grifﬁth energy release parameter j = 1. The imposed vertical displacement at the bottom is increased from 0.02 to 0.08 on a given time interval and shown as abscissa in the ﬁgures. In order to study convergence under mesh reﬁnement, four different meshes are used: 280 280 (coarse), 320 320 (intermediate 1), 400 400 (intermediate 2), 452 452 (ﬁne). Similarly, for convergence under time step reﬁnement, we divide the time interval successively in 100, 200 and 400 time steps. Fig. 1 displays the result for the 320 320 mesh with 100 time steps. There are no subcritical loads: the initiation load coincides with the critical load which means that, not only the appearance of damage is sudden, but the structure completely fails in just one load displacement increment. Fig. 2 shows that the results are convergent under mesh reﬁnements. The curves are almost identical and the position of the critical load is clearly converging as the mesh is reﬁned. Fig. 3 is concerned with convergence under time-step reﬁnement. In particular, the critical loads for the three time reﬁnements show very good agreement, meaning that our quasi-static numerical model seems to converge to a time-continuous model as the time step tends to zero. The cost function (2.4), which is minimized at each time step, is the sum of the Grifﬁth or damage energy and of the elastic energy. The damage energy, displayed in Fig. 2(a), is discontinuous and increases abruptly at the critical load. Similarly, the elastic energy, displayed in Fig. 2(b), is discontinuous decreasing at the critical load, which corresponds to the release of energy produced by damage. However, by comparison, the cost function, displayed in Fig. 2(c), seems to be roughly continuous with respect to time (there is a small bump at the critical load). Eventually, we have checked the following formula for the dissipation of energy (see Theorem 4.1 in [31])

min J ðu; vÞðTÞ min J ðu; vÞð0Þ ¼ u;v

u;v

Z 0

T

Z CD

ðrnÞ

duD ðtÞ dS dt; dt

ð6:1Þ

Fig. 1. Mode I damage for the 320 320 mesh with 100 time steps. Initial conﬁguration with an imposed displacement of 0.02 (a) critical load at an imposed displacement of 0.06 (b) and supercritical load with an imposed displacement of 0.072 (c).

5030

G. Allaire et al. / Journal of Computational Physics 230 (2011) 5010–5044

0.9

intermediate1, intermediate2 and fine

0.7 0.5 0.3

coarse

0.1 0.02

0.03

0.04

0.05

0.06

0.07

0.08

2 coarse 1.5

1

0.5 intermediate1, intermediate2 and fine 0.02

0.03

0.04

0.05

0.06

0.07

0.08

3

2 coarse

1

intermediate1, intermediate2 and fine 0 0.02

0.03

0.04

0.05

0.06

0.07

0.08

Fig. 2. Mode I damage experiment: variations of various energies as functions of the imposed displacement. Grifﬁth energy (a), elastic energy (b) and cost function (c) for four different mesh reﬁnements with 100 time steps.

where J is deﬁned by (2.3) and uD is the applied displacement. In the absence of any other applied load, formula (6.1) expresses the conservation of total energy. If we plot the right hand side of (6.1), we obtain exactly the cost function on the left hand side with a numerical precision of the order of 106. 6.2. 2d Fracture with mode I loading We now switch to a very weak damage phase, E0 = 103, in order to mimic crack propagation. Here the Grifﬁth energy release parameter is j = 3.5. We perform the same mode I traction experiment as in Section 6.1 with the same parameter

5031

G. Allaire et al. / Journal of Computational Physics 230 (2011) 5010–5044

3

2.5

100

2 400

1.5 200

1

0.5

0.02

0.03

0.04

0.05

0.06

0.07

0.08

Fig. 3. Mode I damage experiment: cost function with respect to the imposed displacement for the 320 320 mesh and for 100, 200 and 400 time steps.

values otherwise explicitly speciﬁed. For a mesh of size 320 320, with an initial crack having a width of 8 mesh cells, a height of 16, and for 100 time steps, when the imposed vertical displacement at the bottom is increased from 0.005 to 0.05, we obtain a crack which breaks the structure in just one time increment (see Fig. 4). For all other values of the parameters, the same qualitative behavior is observed: the initial and critical loads are the same for a mode I crack.

Fig. 4. Mode I crack: initial conﬁguration (a) and critical load at 0.0028 (b).

0.4 0.35 0.3 0.25 100, 200 and 400

0.2 0.15 0.1 0.05 0 0.005

0.01

0.015

0.02

0.025

0.03

0.035

0.04

0.045

0.05

Fig. 5. Time-step reﬁnement for the mode I crack: cost function with respect to the imposed displacement for three time reﬁnements.

5032

G. Allaire et al. / Journal of Computational Physics 230 (2011) 5010–5044

We then investigate the convergence under time-step reﬁnement (Fig. 5). The imposed vertical displacement at the bottom is increased from 0.005 to 0.05. The time interval is successively divided in 100, 200 and 400 time steps. The mesh is of size 320 320 with an initial crack having a width of 8 mesh cells. In Fig. 5 the values of the critical loads are obviously converging as Dt goes to zero. Therefore we believe that our quasi-static numerical model, as applied to ‘‘crack-like’’ damage, also converges to a time-continuous model as the time step tends to zero. We now perform three different test cases of convergence under mesh reﬁnement with four meshes for each test (see Figs. 6–8). The four different meshes are: 280 280 (coarse), 320 320 (intermediate 1), 400 400 (intermediate 2), 452 452 (ﬁne). From these three reﬁnement processes, only the last one is fully satisfactory but the two previous ones are illuminating so we keep them in our exposition. In the ﬁrst case (Fig. 6), the given initial crack has a constant width. In other words, the number of cells in a cross-section of the initial crack is 6, 8, 10 and 12, respectively for the four different meshes. The initial crack tip is slightly rounded for the ﬁner meshes in order to avoid the appearance of sharp corners. The imposed vertical displacement at the bottom is increased from 0.005 to 0.05. In Fig. 6 we observe that the value of the critical load is decreasing as the mesh is reﬁned and does not seem to converge (especially when compared to the damage case in Fig. 2). Similarly, the value of the cost function at the critical load is decreasing with ﬁner meshes because a thinner crack (on a ﬁner mesh) costs less Grifﬁth energy. Therefore, contrary to the damage experience of Subsection 6.1, no mesh convergence can be claimed in this ﬁrst experiment. In the second case (Fig. 7), we anticipate that a crack should have a thickness of the order of a few cells Dx when Dx goes to zero. Therefore, whatever the value of Dx, the initial crack is chosen with a width of two cells only, which means that the

0.45 0.4 coarse

0.35 0.3

intermediate 1

0.25 0.2 fine

0.15 0.1 0.05 0 0.005

intermediate 2

0.01

0.015

0.02

0.025

0.03

0.035

0.04

0.045

0.05

Fig. 6. First mesh convergence test for the mode I crack: cost function with respect to the imposed displacement for various meshes and with 100 time steps.

0.6 0.5 intermediate 1

0.4 0.3 coarse fine

0.2 0.1

intermediate 2

0 0.005

0.01

0.015

0.02

0.025

0.03

0.035

0.04

0.045

0.05

Fig. 7. Second mesh convergence test for the mode I crack: cost function with respect to the imposed displacement for various meshes and with 100 time steps.

5033

G. Allaire et al. / Journal of Computational Physics 230 (2011) 5010–5044

0.45 0.4 0.35

fine

0.3 intermediate 2

0.25 0.2 0.15 0.1

coarse and intermediate 1

0.05 0 0.005

0.01

0.015

0.02

0.025

0.03

0.035

0.04

0.045

0.05

Fig. 8. Third mesh convergence test for the mode I crack: cost function (2.11) with respect to simultaneous mesh, crack and j reﬁnements for 100 time steps.

initial crack is thinner and thinner as the mesh is reﬁned. The imposed vertical displacement at the bottom is now increased from 0.005 to 0.05. Reﬁnements with respect to the mesh size are shown in Fig. 7. The critical load again occurs sooner for ﬁner meshes, thereby indicating that there is no convergence under mesh reﬁnement. In the third case (Fig. 8), we replace the minimization of (2.4) by that of the scaled cost function (2.11) in an attempt to show that there is indeed convergence under mesh reﬁnement. In other words we replace the Grifﬁth energy release parameter j by its scaled version Dcx ¼ Djx‘ where Dx is the mesh size. We again choose E0/E1 = 106 and take ‘ = 1/320 (so that ‘/Dx = 1 for the ‘‘intermediate 1’’ mesh). In practice, this scaling implies that it is more difﬁcult to create damage for ﬁner meshes, a phenomenon that should balance the opposite effect displayed in the two previous cases. As explained in Section 2.3 this scaling is precisely designed so the scaled Grifﬁth energy converges to a surface energy when Dx goes to zero. In Fig. 8 we check that the critical loads are converging, so we claim that mesh convergence is observed with this particular scaling of j. Eventually, we have again checked the balance of energy expressed in (6.1): the cost function perfectly matches the time integral of the dissipated energy (i.e. the right hand side of (6.1)), up to a numerical precision of the order of 106. 6.3. 2d fracture with mode II loading We now turn to another crack experiment with a mode II loading. The dimensions of the computational domain are the same as in the above mode I experiments. The weak damage phase is again E0 = 106 while the imposed horizontal displacement at the bottom is here increased from 0.1 to 1.0 on a given time interval. In Fig. 9(a) and (b) the initial and critical cracks are shown for the 320 320 mesh. We emphasize that ‘‘critical’’ has not exactly the same meaning here as for the mode I crack: the mode II crack does not actually break the structure. The crack stops just a few cells before reaching the opposite boundary and does not move anymore as the load increases. This longest crack conﬁguration is called critical. However, fracture is here again brutal in the sense that the initiation load coincides with the critical load. In Fig. 9 we can see that the mode II loading yields a branching of the crack. By symmetry and since the model is linearized elasticity the two crack branches are

Fig. 9. Mode II crack experiment: initial conﬁguration (a) and critical load at 0.49 (b).

5034

G. Allaire et al. / Journal of Computational Physics 230 (2011) 5010–5044

symmetric, one in compression and the other in traction. It means that another mechanical model taking into account the non-interpenetration of material would produce only the branch under traction, i.e., the lips of which are opening under the load, as it can be observed in physical experiments. Four different meshes are used: 280 280 (coarse), 320 320 (intermediate 1), 400 400 (intermediate 2), 452 452 (ﬁne). In our experiment (Fig. 10), we minimize the scaled version (2.11) of the cost function, i.e., j is replaced by Djx‘, and the crack width is always exactly two mesh cells. Convergence under mesh reﬁnement is clearly obtained. Even more, the two ﬁnest mesh curves almost coincide. 6.4. Bittencourt’s drilled plate This test case has been proposed in [16] where we found all the required numerical values of the parameters. It has been reproduced in many other works, including [18,13]. The Young modulus of the healthy phase is 3000 and its Poisson ratio 0.35. The damaged phase has a Young modulus 3 103 and the same Poisson ratio. The value of the Grifﬁth energy release parameter is j = 0.0014. Contrary to all other numerical simulations in this paper, the present experiment has been

30

25

coarse

20

intermediate 1

15 intermediate 2 and fine 10

5

0 0.1

0.2

0.3

0.4

0.5

0.6

0.7

0.8

0.9

1

Fig. 10. Mode II crack test: cost function (2.11) with respect to simultaneous mesh, crack and j reﬁnements for 100 time steps.

Fig. 11. The two Bittencourt’s experiments: (a) ﬁrst case a = 6, b = 1.5 and (b) second case a = 5, b = 1.

G. Allaire et al. / Journal of Computational Physics 230 (2011) 5010–5044

5035

performed with a given ﬁxed applied force instead of a sequence of increasing displacements. The vertical unit load is applied on a single concentrated point of the upper body boundary. The value of the Grifﬁth energy release parameter j is such that this applied unit load is critical, i.e. a single time step produces the cracks displayed in Fig. 11(a) and (b) for two different crack initializations. The distance from the left face to the initial crack is denoted by a, while b is the initial crack length. The three holes carry a Neumann boundary condition. We use a non-uniform rectangular mesh of size 470 800 which is more reﬁned in the vicinity of the holes. These two results are in good agreement with laboratory experiment of [16], although that of Fig. 11(a) shows a slightly different crack path near the second hole. 6.5. Coalescence of multiple cracks This experiment is made on a pre-cracked sample (of size 1.6 2.2) with a vertical imposed displacement along the vertical sides (corresponding to a Mode II type loading). The healthy material has Young modulus E1 = 1 and Poisson ratio m1 = 0.3, the damaged phase has the same Poisson ratio but a smaller Young modulus E0 = 103. The value of the Grifﬁth energy release parameter is j = 107. The imposed vertical displacement is increased from 0.001 to 0.005 with 100 time steps. The critical load is attained at 0.0014. Two different meshes are shown in Fig. 12.

Fig. 12. Multiple crack experiment with a Mode II loading.

Fig. 13. Fiber-reinforced matrix: isocontours of the topological derivative at the initialization.

5036

G. Allaire et al. / Journal of Computational Physics 230 (2011) 5010–5044

6.6. Traction experiment on a ﬁber reinforced matrix We perform a test case proposed in [20] where all precise values of the parameters can be found. The setting of Fig. 14(a) is the following. A unit vertical displacement is exerted on the upper layer of the solid which is also clamped at its midpoint to avoid translations and rotations. The ﬁber (grey inclusion in Fig. 14(a)) is also clamped. The healthy material has Young modulus E1 = 1000 and Poisson ratio m1 = 0.3, the damaged phase has the same Poisson ratio but a much smaller Young modulus E0 = 103. The value of the Grifﬁth energy release parameter is j = 8000. Excellent agreement with the numerical results of [20] are observed. Let us emphasize that this experiment is the only one using the topological derivative to initiate the damaged zone: the map of the topological gradient at the initialization is displayed in Fig. 13. More precisely, the initial body is completely healthy without any damage: the applied load is gradually increased, until damage appears because the topological derivative becomes negative. Once the damaged zone has been initialized we use our shape gradient method to propagate the crack without further use of the topological gradient. The ﬁnal crack in Fig. 14 is very similar to that computed in [20]. There is a subtle point here in the use of the topological derivative. Such a notion is well deﬁned for the cost function (2.3) which features a bulk Grifﬁth-type energy. However, it is not possible to deﬁne a topological derivative for the cost function (2.13) which has a surface Grifﬁth energy. Indeed, surface energy asymptotically dominates bulk energy for small inclusions and no balance can be established. In other words the notion of topological derivative makes sense in our damage model but is irrelevant for fracture models.

Fig. 14. Fiber-reinforced matrix: an example of crack initiation by the topological derivative.

G. Allaire et al. / Journal of Computational Physics 230 (2011) 5010–5044

5037

Note also that the initialization pattern suggested by the topological derivative (which is necessarily small by deﬁnition) is not a local minimizer of the cost function. Thus, such an initialization is difﬁcult to compare with other ones in the literature and its small extension is not a contradiction with theoretical results [28] stating that an initial crack (minimizing the cost function) cannot be too small. Therefore we now compare different (10) initializations for the same problem. The ﬁrst initialization is that given by the topological gradient and already displayed in Fig. 14(b). The nine other ones, displayed in Fig. 15, are increasingly larger cracks obtained as intermediate inner iterates in the previous computation (they are therefore not local minimizers of the cost function). The larger cracks of Fig. 15 are very similar to the initial crack pattern in [21]. For each of these initial cracks we restarted the crack evolution from a zero imposed displacement which is then gradually increased. The evolutions of the elastic energy, the Grifﬁth energy and the cost function, when the imposed displacement is increased, are shown in Fig. 16. One can clearly see the importance of the initialization, a well-known fact in the minimization of non-convex energies. The idea of restarting the minimization at smaller loading parameters from an intermediate crack solution at a larger loading parameter has already been exploited in the so-called back-tracking algorithm of [19,21] for global minimization. Of course, the larger the initial crack is, the smaller is the critical load. Interestingly enough we found that, for the 4th up to the 10th initializations, part of the crack evolution is smooth with respect to the loading parameter. This is actually the only occurrence in our numerical tests of a continuous crack evolution: all other examples feature a brutal fracture process. This smooth behavior is very similar to that obtained in [21] (see Figs. 31 and 32 on p. 92). In Fig. 17, for the 5th initialization, we plot the two crack patterns obtained for the values 0.28 and 0.44 of the imposed displacement: in between the crack evolution is continuous. 6.7. 3d mode 1, mode 2 and mode 3 cracks We eventually conclude our numerical tests by performing the 3 different mode loadings in 3d with boundary conditions (imposed displacements) shown in Fig. 18. We work with a cubic domain of size 1 1 1 meshed with 80 80 80 cubic

Fig. 15. Fiber-reinforced matrix: different crack initializations.

5038

G. Allaire et al. / Journal of Computational Physics 230 (2011) 5010–5044

300 250 200 150 100 50 0 0

0.1

0.2

0.3

0.4

0.5

0.6

0.7

0.8

0

0.1

0.2

0.3

0.4

0.5

0.6

0.7

0.8

0

0.1

0.2

0.3

0.4

0.5

0.6

0.7

0.8

80

40

0

300 250 200 150 100 50 0

Fig. 16. Elastic energy, Grifﬁth energy and cost function, as a function of the imposed displacement, for the 10 initializations of Fig. 15. The ﬁrst initialization corresponds to the largest critical load (or discontinuity) and the critical load is decreasing with the label of the initialization.

cells: its left back face (circles) is ﬁxed while a uniform displacement of modulus 0.04 is applied on its right front face. The healthy material has Young modulus E1 = 104 and Poisson ratio m1 = 0.3, the damaged phase has the same Poisson ratio but a smaller Young modulus E0 = 1. The value of the Grifﬁth energy release parameter is j = 1. The initial and ﬁnal cracks are shown in Fig. 19. For this large test case (involving around 1.56 106 degrees of freedom) we use a sparse parallel direct linear solver for solving the elasticity system, requiring 40 GB of memory and 15 min on 8 Intel Xeon processors. Each of these 3d

G. Allaire et al. / Journal of Computational Physics 230 (2011) 5010–5044

5039

Fig. 17. Fiber-reinforced matrix: two crack patterns for the 5th initialization at the beginning and at the end of a smooth evolution.

Fig. 18. Boundary conditions for the modes I, II and III in 3d.

computations requires of the order of 150 and 200 iterations, i.e. solutions of the elasticity system, so the overall CPU time is about two days. 7. Concluding remarks We have proposed a numerical method, based on the Francfort–Marigo damage model and using a single level set function with standard ﬁnite elements, for the simulation of damage evolution and crack propagation. Our method is computing

5040

G. Allaire et al. / Journal of Computational Physics 230 (2011) 5010–5044

Fig. 19. Initial and ﬁnal cracks for the modes I, II and III in 3d.

a class of local minimizers of the Francfort–Marigo energy. The crack paths predicted by our numerical experiments are in excellent qualitative agreement with previous results in the literature. However, the quasi-static evolutions of the elastic energy, Grifﬁth-type damage energy and total cost function are different from those we found in [21] (using global minimization), and in [48] (using criticality). First, cracks often break the structure in a single time increment: fracture is thus a brutal process in most of our computations, which is not the case in [21,48]. Second, as opposed to the global minimization approach of [21], the cost function (which is the sum of the elastic and damage energies) is not continuous in time: at the critical load (when the structure breaks down) some energy is thus dissipated. This phenomenon seems to be featured by all local minimization approaches and is usually interpreted as the necessity of including kinetic effects in the model. The ill-posed character of the minimization problem (2.4) or (2.11) (which do not admit minimizers, in general) manifests itself in various aspects. First, as already said, we rarely found a local minimizer in our numerical tests unless the structure was broken (fracture is a brutal process). The only exception is the ﬁber reinforced matrix test of Section 6.6 where a larger than usual initial crack allows us to obtain a smooth evolution of the crack, similar to that obtained in [21]. Second, our numerical results are quite sensitive to some implementation issues. For example, it is necessary to use the complete shape derivative formulas (3.9) (which features the two phases) and not their simpler limit (3.13), obtained when the damaged phase is assumed to have zero rigidity, otherwise the minimization of the cost function is less complete and the values of the initiation or critical loads may be wrong. Another important issue is the reinitialization process which must be precise enough so that the normal and tangent vectors to the interface between the two phases are always accurately computed while the interface itself does not move at all during reinitialization (otherwise it would contradict the irreversibility constraint). An interesting open problem is to prove the conjectured convergence of the discrete scaled energy (2.12) towards the fracture model (2.13). A natural extension of our work is to handle a non-interpenetration condition so that cracks under compression do not propagate. We have used standard Q1 ﬁnite elements for solving the linear elasticity system which features a large variation of the Young modulus between the two phases. It would be interesting to study if extended ﬁnite element methods (XFEM, see e.g. [36,37]) would improve the numerical precision at a not too large expense in CPU cost. Of course, we should also perform more realistic test cases and make precise comparisons with both physical experiments and other codes, including a study of CPU cost. Eventually let us mention that shape optimization for minimizing the risk of crack propagation is also a promising ﬁeld to investigate, following [45].

5041

G. Allaire et al. / Journal of Computational Physics 230 (2011) 5010–5044

Acknowledgments This work has been supported by the MULTIMAT European network MRTN-CT-2004–505226 funded by the EEC. G. Allaire is a member of the DEFI project at INRIA Futurs Saclay and is partially supported by the Chair ‘‘Mathematical modelling and numerical simulation, F-EADS – Ecole Polytechnique – INRIA’’ and by the GNR MoMaS sponsored by ANDRA, BRGM, CEA, CNRS, EDF, and IRSN. G. Allaire and F. Jouve were partly supported by the ANR project MICA, ANR-06-BLAN-0082. N. Van Goethem was partly supported by the Fundação para a Ciência e a Tecnologia (Ciência 2007 and FCT Project: PTDC/EMEPME/108751/2008). The authors thank the reviewers for their constructive comments. Appendix A. Computation of the shape derivative This appendix is devoted to the proofs of Lemma 3.6 and Corollary 3.1. We begin with Lemma 3.6 which furnishes the partial shape derivative of the Lagrangian. To prove it we use Lemma 3.1. On the one hand, the derivatives of integrals on X0,1 are simple. On the other hand, the interface R is either a closed surface without boundary or a surface which meets the outer boundary @ X: in both cases the derivative of an integral on R has no contribution on its boundary @ R as in (3.1). Eventually, even if the 0;1 surfaces C0;1 N are subset of the ﬁxed boundary CN, they can vary tangentially to CN, so the derivatives of integrals on CN are made of the sole boundary term on c ¼ @ C0;1 in (3.1). Therefore, the partial shape derivative of L is N

@L h ; /i ¼ @v

Z

R

þ

1 2

r1 ðu1 Þ eðp1 Þ r0 ðu0 Þ eðp0 Þ h n dS þ

Z 1 0 f 1 p1 þ f 0 p0 j ðu1 Þ þ j ðu0 Þ h n dS R

Z

ðr0 ðu0 Þ eðu0 Þ r1 ðu1 Þ eðu1 ÞÞh n dS

R

1 2

Z R

@ þ H ððr1 ðp1 Þn þ r0 ðp0 ÞnÞ ðu1 u0 ÞÞh n dS R @n Z Z 1 @ 0 1 þ þ H ððr1 ðu1 Þn þ r0 ðu0 ÞnÞ ðu1 u0 ÞÞh nk dS þ ðg 0 p0 g 1 p1 þ h ðu0 Þ h ðu1 ÞÞh sdL; 2 R @n c 1 2

Z

@ þ H ððr1 ðu1 Þn þ r0 ðu0 ÞnÞ ðp1 p0 ÞÞh n dS @n

ðA:1Þ where H denotes the mean curvature and s is the external unit vector normal to c = @ CN and n. Since u0 = u1 and p0 = p1 on R, the terms involving the curvature vanish on R. Similarly the normal component of the stress tensors are continuous through R. Thus, (A.1) simpliﬁes in

@L h ; /i ¼ @v

Z

Z 1 0 0 ðr ðu Þ eðu0 Þ r1 ðu1 Þ eðu1 ÞÞh n dS rðuÞn R R 2 R Z Z Z @ðp1 p0 Þ @ðu1 u0 Þ @ðu1 u0 Þ h n dS rðpÞn h n dS þ rðuÞn h n dS ððf 1 f 0 Þ p @n @n @n R R R Z 1 0 1 0 þ j ðuÞ j ðuÞÞh n dS ððg 1 g 0 Þ p þ h ðuÞ h ðuÞÞh sdL; ðr1 ðu1 Þ eðp1 Þ r0 ðu0 Þ eðp0 ÞÞh n dS þ

Z

ðA:2Þ

c

where u, p, r(u)n, r(p)n denotes the continuous quantities at the interface. The two last lines of (A.2) are expressed only in terms of continuous quantities through the interface, but not the ﬁve ﬁrst lines that we must rewrite, using Lemma 3.2, as an explicit expression in terms of continuous functions at the interface and jumps of the Lamé coefﬁcients. (In the following computations, the symbol will denote, according to the context, either a scalar product between two vectors, or between two matrices.) Let us compute the integrand in the ﬁrst term of the right hand side of (A.2). In the local orthonormal basis (t, n) (adapted to the interface R and introduced in Lemma 3.2) the following decomposition holds

r1 ðu1 Þ eðp1 Þ ¼ r1nn ðu1 Þenn ðp1 Þ þ 2r1tn ðu1 Þ etn ðp1 Þ þ r1tt ðu1 Þ ett ðp1 Þ: From Lemma 3.2 it rewrites as

r1 ðu1 Þ eðp1 Þ ¼

1 k1 þ 2l1 "

þ 2l1 ett ðu1 Þ þ ¼

1 1

k þ 2l

r1nn ðu1 Þ r1nn ðp1 Þ k1 trett ðp1 Þ þ k1

k1 þ 2l1

r1 ðu1 Þr1nn ðp1 Þ þ 1 nn

1

l1

r1tn ðu1 Þ r1tn ðp1 Þ

# 2l1 trett ðu1 Þ þ r1nn ðu1 Þ Id1 ett ðp1 Þ 2 1

l

1

r1tn ðu1 Þ r1tn ðp1 Þ þ 2l1 ett ðu1 Þ ett ðp1 Þ þ

2k1 l1 1

k þ 2l1

trett ðu1 Þtrett ðp1 Þ:

5042

G. Allaire et al. / Journal of Computational Physics 230 (2011) 5010–5044

A similar computation with the index 0 instead of 1 yields the difference

r1 ðu1 Þ eðp1 Þ r0 ðu0 Þ eðp0 Þ ¼

1 k þ 2l

rnn ðuÞrnn ðpÞ þ

1

l

rtn ðuÞ rtn ðpÞ þ ½2lett ðuÞ ett ðpÞ þ

2kl trett ðuÞtrett ðpÞ k þ 2l

which is expressed, as desired, only in terms of continuous functions at the interface. On the same token we deduce

r0 ðu0 Þ eðu0 Þ r1 ðu1 Þ eðu1 Þ ¼

1 1 2kl ðrnn ðuÞÞ2 jrtn ðuÞj2 ½2ljett ðuÞj2 ðtrett ðuÞ2 : k þ 2l l k þ 2l

We now consider the integrand of the third, fourth of ﬁfth line of (A.2). We use the following identity for two displacements v and q

rðv Þn

if q ¼ 0 on R; then

@q ¼ 2ðrðv ÞnÞ ðeðqÞnÞ rnn ðv Þenn ðqÞ on R: @n

We obtain

rðuÞn

@ðp1 p0 Þ ¼ 2ðrðuÞnÞ ðeðp1 Þn eðp0 ÞnÞ rnn ðuÞðenn ðp1 Þ enn ðp0 ÞÞ @n 2 2k 1 rnn ðuÞrnn ðpÞ rnn ðuÞtrett ðpÞ þ r ðuÞ rtn ðpÞ ¼ k þ 2l k þ 2l l tn 1 k rnn ðuÞrnn ðpÞ þ rnn ðuÞtrett ðpÞ k þ 2l k þ 2l 1 1 k ¼ rnn ðuÞrnn ðpÞ þ rtn ðuÞ rtn ðpÞ rnn ðuÞtrett ðpÞ: k þ 2l k þ 2l l 1

0

1

ðA:3Þ

0

We get a similar expression for rðpÞn @ðu @nu Þ and rðuÞn @ðu @nu Þ. Summing up these contributions we deduce that the integrand of the ﬁve ﬁrst lines of the right hand side of (A.2) is

1 1 2kl trett ðuÞ trett ðpÞ DðxÞ ¼ rnn ðuÞrnn ðpÞ rtn ðuÞ rtn ðpÞ þ ½2lett ðuÞ ett ðpÞ þ k þ 2l l k þ 2l k 1 1 ðrnn ðuÞtrett ðpÞ þ rnn ðpÞtrett ðuÞÞ þ jrtn ðuÞj2 ½ljett ðuÞj2 þ ðrnn ðuÞÞ2 þ k þ 2l 2ðk þ 2lÞ 2l kl k ðtrett ðuÞÞ2 rnn ðuÞtrett ðuÞ k þ 2l k þ 2l which is precisely formula (3.10). Using the relations (3.8) between e and r (see Lemma 3.2) we easily deduce (3.11) from (3.10), which ﬁnishes the proof of Lemma 3.6. h Proof of Corollary 3.1. The Francfort–Marigo objective function is obtained for jk(u) = f ku + jdk0 and hk(u) = gku. 0 We deduce that j0k ðuÞ ¼ f k and hk ðuÞ ¼ g k , and thus that the adjoint state vanishes pv = 0. If we further assume that 0 1 0 1 f = f and g = g , the shape derivative reduces to

J 0 ðvÞðhÞ ¼

Z

DðxÞ h n dS

R

with

DðxÞ ¼

1 1 kl k jrtn ðuv Þj2 ½ljett ðuv Þj2 rnn ðuv Þtrett ðuv Þ: ðrnn ðuv ÞÞ2 þ ð trett ðuv ÞÞ2 2ðk þ 2lÞ 2l ðk þ 2lÞ ðk þ 2lÞ ðA:4Þ

0

1

Assumption A 6 A is equivalent to [l] P 0 and ½, P 0 with , :¼ k þ l, the bulk modulus. Since rtn(u) only appears as a square product in (A.4), it sufﬁces to check that the combination of all other terms is indeed negative, that is, 2 d

1 2kl 2k ðrnn ðuÞÞ2 ½2ljett ðuÞj2 ðtrett ðuÞÞ2 rnn ðuÞtrett ðuÞ 6 0: k þ 2l k þ 2l k þ 2l

ðA:5Þ

Since (trett(u))2 6 (d 1)jett(u)j2 (where d = 2, 3 is the space dimension) the left hand side of (A.5) is bounded from above by

1 k þ 2l

rnn ðuÞ2

2l 2kl 2k ðtrett ðuÞÞ2 rnn ðuÞtrett ðuÞ; þ k þ 2l d 1 k þ 2l

ðA:6Þ

G. Allaire et al. / Journal of Computational Physics 230 (2011) 5010–5044

5043

which writes in term of , and l as

d d, þ 2ðd 1Þl

rnn ðuÞ2

d 2d,l d, 2l tr2 ett ðuÞ 2 rnn ðuÞtrett ðuÞ: d 1 d, þ 2ðd 1Þl d, þ 2ðd 1Þl

Since, by assumption A0 6 A1, we have

d 2d,l 6 0 and P 0; d, þ 2ðd 1Þl d, þ 2ðd 1Þl

the quadratic form (A.6) is negative if and only if

d, 2l d, þ 2ðd 1Þl

2 6

d d 2d,l : d 1 d, þ 2ðd 1Þl d, þ 2ðd 1Þl

ðA:7Þ

Introducing the new variables ,0 ¼ d2, and l0 = (d 1)l, (A.7) is equivalent to

1 , 0 þ l0

,0 l0 1 ðd 1Þ,0 l0 6 2 0 0 , þl , 0 þ l0 d

2 ¼

2 1 ,0 l0 : 4 ,0 þ l0

ðA:8Þ

A brute force computation shows that (A.8) holds true. h References [1] J. Alfaiate, G.N. Wells, L.J. Sluys, On the use of embedded discontinuity elements with crack path continuity for mode-I and mixed-mode fracture, Eng. Fract. Mech. 69 (2002) 661–686. [2] G. Allaire, Continuity of the Darcy’s law in the low-volume fraction limit, Ann. Scuola Norm. Sup. Pisa 18 (1991) 475–499. [3] G. Allaire, Conception optimale de structures, Collection: Mathématiques et Applications, vol. 58, Springer, 2007. [4] G. Allaire, S. Aubry, F. Jouve, Simulation numérique de l’endommagement à l’aide du modèle Francfort–Marigo, in: Actes du 29ème congrès d’analyse numérique, ESAIM Proceedings, vol. 3, pp.1–9, 1998. [5] G. Allaire, F. Jouve, A.-M. Toader, Structural optimization using sensitivity analysis and a level-set method, J. Comput. Phys. 194 (1) (2004) 363–393. [6] G. Allaire, F. Jouve, N. Van Goethem, A level set method for the numerical simulation of damage evolution, in: R. Jeltsch, G. Wanner (Eds.), Proceedings of ICIAM 2007, Zürich, EMS, Zürich, 2009. [7] L. Ambrosio, V. Tortorelli, Approximation of functionals depending on jumps by elliptic functionals via C-convergence, Commun. Pure Appl. Math. 43 (8) (1990) 999–1036. [8] H. Ammari, H. Kang, Reconstruction of small inhomogeneities from boundary measurements, Lecture Notes in Mathematics, vol. 1846, Springer, 2000. [9] H. Ammari, H. Kang, G. Nakamura, K. Tanuma, Complete asymptotic expansions of solutions of the system of elastostatics in the presence of an inclusion of small diameter and detection of an inclusion, J. Elasticity 67 (2) (2002) 97–129. [10] H. Ammari, An introduction to mathematics of emerging biomedical imaging, Collection: Mathématiques et Applications, vol. 62, Springer, 2008. [11] H. Ammari, P. Calmon, E. Iakovleva, Direct elastic imaging of a small inclusion, SIAM J. Imaging Sci. 1 (2008) 169–187. [12] L. Ambrosio, G. Buttazzo, An optimal design problem with perimeter penalization, Calc. Var. 1 (1993) 55–69. [13] P. Areias, J. Alfaiate, D. Dias-da-Costa, E. Julio, Arbitrary bi-dimensional ﬁnite strain crack propagation, Comput. Mech. 45 (1) (2009) 61–75. [14] P.-E. Bernard, N. Moës, C. Stolz, N. Chevaugeon, A thick level set approach to model evolving damage and transition to fracture, in: Proceedings of ECCM 2010, Paris, May 16–21, 2010. [15] Ch. Bernardi, O. Pironneau, Sensitivity of Darcy’s law to discontinuities, Chinese Ann. Math. Ser. B 24 (2) (2003) 205–214. [16] T.N. Bittencourt, A.R. Ingraffea, P.A. Wawrzynek, J.L. Sousa, Quasi-automatic simulation of crack propagation for 2D LEFM problems, Eng. Fract. Mech. 55 (2) (1996) 321–324. [17] M. Bonnet, A. Constantinescu, Inverse problems in elasticity, Inverse Problems 21 (2005) 1–50. [18] S. Bordas, B. Moran, Enriched ﬁnite elements and level sets for damage tolerance assessment of complex structures, Eng. Fract. Mech. 73 (9) (2006) 1176–1201. [19] B. Bourdin, Numerical implementation of the variational formulation for quasi-static brittle fracture, Interface Free Bound 9 (2007) 411–430. [20] B. Bourdin, G.A. Francfort, J.-J. Marigo, Numerical experiments in revisited brittle fracture, J. Mech. Phys. Solids 48 (4) (2000) 797–826. [21] B. Bourdin, G.A. Francfort, J.-J. Marigo, The variational approach to fracture, Journal of Elasticity 91 (2008) 5148. [22] A. Braides, C. Larsen, C-convergence for stable states and local minimizers, preprint. [23] A. Braides, A. Piatnitski, Homogenization of surface and length energies for spin systems, preprint. Available at

5044

G. Allaire et al. / Journal of Computational Physics 230 (2011) 5010–5044

[39] F. Hettlich, W. Rundell, The determination of a discontinuity in a conductivity from a single boundary measurement, Inverse Problems 14 (1) (1998) 67–82. [40] R. Jerrard, P. Sternberg, Critical points via Gamma-convergence: general theory and applications, J. Eur. Math. Soc. 11 (2009) 705–753. [41] C. Larsen, Epsilon-stable quasi-static brittle fracture evolution, Commun. Pure Appl. Math. 63 (2010) 630–654. [42] C. Larsen, C. Richardson, M. Sarkis, A level set method for the Mumford-Shah functional and fracture, SIAM J. Imag. Sci., in press. Available from:

Copyright © 2024 C.COEK.INFO. All rights reserved.